Materials Testing Results - Paints and Sealants

==Paints and Sealants==
Material Name 	Manufacturer 	Supplier 	Test Results 	Date tested 	Tester	Test(s) Used 	Description/ Composition 	Comments 	Material Type 	Results Image or Description 	
KEIM Optil White paint 	KEIM 	KEIM 	FAIL 	2022/02/15 	MMA 	Oddy Test (method: 20211201_OT ) 	Ready to use silica-sol interior mineral paint in accordance with DIN EN 3 300; pH ~11, 1.3-1.6 g/mL density; aqueous solution of silicic acid potassium salt and/or silica sol, acrylic polymer, mineral fillers, pigments, additives. Contains 2-methylisothiazol-3(2H)-one; applied to aluminum foil and allowed to cure for 3 weeks (21 days), tested on foil; Purchased September 2020, new liquid sample from Michael Dominick December 2021 	 	-Coating - paint or primer 	 	
Ultraspec 500 Interior Flat Finish N536, "OC-152" Super White paint 	Benjamin Moore 	Benjamin Moore 	FAIL 	2022/02/15 	MMA 	Oddy Test (method: 20211201_OT ) 	White waterborne flat finish paint based on a proprietary cross-linking acrylic resin that tints on the Gennex® zero VOC colorant system; 1.31-1.36 g/mL density, 100°C boiling point; contains titanium dioxide, limestone, diatomaceous earth, and kaolin, calcined; applied to aluminum foil and allowed to cure for 3 weeks (21 days), tested on foil; Purchased September 2020, new liquid sample from Michael Dominick December 2021 	 	-Coating - paint or primer 	 	
Ultraspec HP D.T.M. Acrylic Low Luster Enamel HP25, "OC-152" Super White paint 	Benjamin Moore 	Benjamin Moore 	FAIL 	2022/02/15 	MMA 	Oddy Test (method: 20211201_OT ) 	White paint designed to perform a dual purpose as a direct to metal primer and finish; 1.18-1.23 g/mL density, 100°C boiling point; contains titanium dioxide, zinc phosphate, 2,2,4-trimethyl-1,3-propanediol diisobutyrate, and kaolin; applied to aluminum foil and allowed to cure for 3 weeks (21 days), tested on foil; Purchased September 2020, new liquid sample from Michael Dominick December 2021 	 	-Coating - paint or primer 	 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Medium #1671 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: no change 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Ultra #042 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: no change 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Ultra #042 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: no change 	
BM Super Spec Latex Vapor Barrier Primer Sealer 260 on Appleply 	Benjamin Moore Appleply:States Industries 	 	fail 	2006/03/22 	NMAI 	Oddy Test 	 	A-D strip test fail 	coating 	Cu: gold/yellow tone; Ag: no change; Pb: thick white crystals, yellow at exterior tip 	
BM Super Spec Latex Vapor Barrier Primer Sealer 260 on Appleply 	Benjamin Moore; Appleply:States Industries 	 	fail 	2006/03/22 	NMAI 	Oddy Test 	 	A-D strip test fail 	coating 	Cu: gold/yellow tone; Ag: no change; Pb: thick white corrosion all over; yellow crystals on underside of coupon 	
BM Fresh Start All-Purpose Alkyd Primer 024 on Appleply 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2006/02/13 	NMAI 	Oddy Test 	 	A-D strip test pass 	coating 	Cu: slightly dark orange; Ag: no change; Pb: white corrosion product all over; thick crystal buildup 	
BM Fresh Start All-Purpose Alkyd Primer 024 on Appleply 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2006/02/13 	NMAI 	Oddy Test 	 	A-D strip test pass 	coating 	Cu: slightly dark orange; Ag: no change; Pb: white powdery surface all over; small crystal buildup 	
BM Fresh Start All-Purpose Alkyd Primer 024 on mylar 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2006/02/13 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: white/yellow/grey powdery surface all over 	
BM Fresh Start All-Purpose Alkyd Primer 024 on mylar 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2006/02/13 	NMAI 	Oddy Test 	 	 	coating 	Cu: dark orange; Ag: no change; Pb: white/yellow thick powdery surface all over 	
BM Super Spec Latex Vapor Barrier Primer Sealer 260 on mylar 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/02/13 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: darkened 	
BM Super Spec Latex Vapor Barrier Primer Sealer 260 on mylar 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/02/13 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: light layer of light blue/grey powdery surface corrosion 	
Ben. Moore Platinum Epoxy M42 on Appleply 	Benjamin Moore www.benjaminmoore.com 	 	Fail 	2005/10/05 	NMAI 	Oddy Test 	 	this was a retest; previous test number 2005-08-01; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge; A-D strip test: 1 out of scale 0 (pass) to 3 (fail) 	coating 	Cu: darkened; Ag: no change; Pb: white corrosion overall; some buildup at edge 	
Ben. Moore Platinum Epoxy M42 on Appleply 	Benjamin Moore www.benjaminmoore.com 	 	Fail 	2005/10/05 	NMAI 	Oddy Test 	 	this was a retest; previous test number 2005-08-02; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge; A-D strip test: 1 out of scale 0 (pass) to 3 (fail) 	coating 	Cu: darkened; Ag: no change; Pb: white corrosion overall; some buildup 	
Sancure on Appleply (2 coats) 	Sancure: Noveon. Appleply: States Industries 	 	Fail 	2005/10/05 	NMAI 	Oddy Test 	 	this was a retest; previous test number 2005-08-03; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge.; A-D strip test: 0.5 out of scale 0 (pass) to 3 (fail) 	coating 	Cu: no change/ very slightly darkened; Ag: no change; Pb: white corrosion overall 	
Sancure on Appleply (2 coats) 	Sancure: Noveon. Appleply: States Industries 	 	Fail 	2005/10/05 	NMAI 	Oddy Test 	 	this was a retest; previous test number 2005-08-04; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge; A-D strip test: 0.5 out of scale 0 (pass) to 3 (fail) 	coating 	Cu: no change/ very slightly darkened; Ag: no change; Pb: white corrosion overall 	
FoamBlast 349 	Lubrizol Foam Control Additives www.lubrizol.com 	 	pass 	2005/10/05 	NMAI 	Oddy Test 	 	Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge; A-D strip test pass 	coating 	Cu: slightly darkened/ irridescent; Ag: no change; Pb: darkened; white spot from condensation 	
FoamBlast 349 	Lubrizol Foam Control Additives www.lubrizol.com 	 	pass 	2005/10/05 	NMAI 	Oddy Test 	 	Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge; A-D strip test pass 	coating 	Cu: slightly darkened/ irridescent; Ag: no change; Pb: darkened 	
Microsol 2030 Accent Base 	Breathe EZ Best Paint Co. www.bestpaintco.com 	 	pass 	2005/10/05 	NMAI 	Oddy Test 	 	Microsol paints allowed 1 week to offgas; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge. 	coating 	Cu: slightly darkened; Ag: no change; Pb: darkened; spot of white corrosion product possibly from condensation 	
Microsol 2030 Accent Base 	Breathe EZ Best Paint Co. www.bestpaintco.com 	 	pass 	2005/10/05 	NMAI 	Oddy Test 	 	Microsol paints allowed 1 week to offgas; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge. 	coating 	Cu: slightly darkened; Ag: no change; Pb: darkened; spot of white corrosion product possibly from condensation 	
Microsol 2030 Pastel Base 	Breathe EZ Best Paint Co. www.bestpaintco.com 	 	pass 	2005/10/05 	NMAI 	Oddy Test 	 	Microsol paints allowed 1 week to offgas; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge. 	coating 	Cu: irridescent overall, darkened severely on 1/2 interior of coupon; Ag: no change; Pb: darkened 	
Microsol 2030 Pastel Base 	Breathe EZ Best Paint Co. www.bestpaintco.com 	 	pass 	2005/10/05 	NMAI 	Oddy Test 	 	Microsol paints allowed 1 week to offgas; Control: Cu - darkened, Ag - no change, Pb - darkened, blue tinge. 	coating 	Cu: irridescent, darkened overall; Ag: no change; Pb: darkened; spot of white corrosion product possibly from condensation 	
Benjamin Moore M42 clear epoxy on Mylar 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2005/08/16 	NMAI 	Oddy Test 	 	retested Cu and Pb only, A-D strip test pass 	coating 	Cu: no change; Pb: no change 	
Benjamin Moore M42 clear epoxy on Mylar 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2005/08/16 	NMAI 	Oddy Test 	 	retested Cu and Pb only, A-D strip test pass 	coating 	Cu: no change; Pb: no change 	
Benjamin Moore M42 clear epoxy on Sintra 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2005/08/16 	NMAI 	Oddy Test 	 	retested Cu and Pb only, A-D strip test pass 	coating 	Cu: no change; Pb: no change 	
Benjamin Moore M42 clear epoxy on Sintra 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2005/08/16 	NMAI 	Oddy Test 	 	retested Cu and Pb only, A-D strip test pass 	coating 	 	
Benjamin Moore M42 platinum gray epoxy on mylar 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2005/08/12 	NMAI 	Oddy Test 	 	noticeable odor on opening jar 	coating 	Cu: no change; Ag: no change; Pb: darkened 	
Benjamin Moore clear epoxy on Appleply (2 coats) 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2005/08/12 	NMAI 	Oddy Test 	 	As vapor barrier for wood product. compared to appleply uncoated and to appleply coated with Sancure 878 and BM platinum epoxy. In this test, they all failed. But Sancure and BM gray reported as passed in context and due to tests by others, A-D strip test: 0.5	coating 	Cu: no change; Ag: no change; Pb: minimal scattered white corrosion 	
Benjamin Moore clear epoxy on Appleply (2 coats) 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2005/08/12 	NMAI 	Oddy Test 	 	As vapor barrier for wood product. compared to appleply uncoated and to appleply coated with Sancure 878 and BM platinum epoxy. In this test, they all failed. But Sancure and BM gray reported as passed in context and due to tests by others, A-D strip test: 0.5	coating 	Cu: no change; Ag: no change; Pb: second coupon completely covered with voluminous yellow corrosion 	
Benjamin Moore platinum gray epoxy on Appleply (2 coats) 	Benjamin Moore www.benjaminmoore.com 	 	Fail 	2005/08/12 	NMAI 	Oddy Test 	 	As vapor barrier for wood product. compared to appleply uncoated and to appleply coated with Sancure 878 and BM clear epoxy. In this test, they all failed. But Sancure and BM gray reported as passed in context and due to tests by others. 	coating 	Cu: no change; Ag: no change; Pb: white and yellow crusty corrosion 	
Benjamin Moore platinum gray epoxy on Appleply (2 coats) 	Benjamin Moore www.benjaminmoore.com 	 	Fail 	2005/08/12 	NMAI 	Oddy Test 	 	As vapor barrier for wood product. compared to appleply uncoated and to appleply coated with Sancure 878 and BM clear epoxy. In this test, they all failed. But Sancure and BM gray reported as passed in context and due to tests by others. 	coating 	Cu: no change; Ag: no change; Pb: white and yellow crusty corrosion 	
Sancure 878 on Appleply (2 coats) 	Sancure: Noveon. Appleply: States Industries 	 	Fail 	2005/08/12 	NMAI 	Oddy Test 	 	As vapor barrier for wood product. Compared to appleply uncoated and to appleply coated with BM epoxies. In this test, they all failed. But Sancure and BM gray reported as passed in context and due to tests by others, A-D strip test: 0.2 	coating 	Cu: no change; Ag: no change; Pb: voluminous white corrosion, heterogeneous 	
Sancure 878 on Appleply (2 coats) 	Sancure: Noveon. Appleply: States Industries 	 	Fail 	2005/08/12 	NMAI 	Oddy Test 	 	As vapor barrier for wood product. Compared to appleply uncoated and to appleply coated with BM epoxies. In this test, they all failed. But Sancure and BM gray reported as passed in context and due to tests by others, A-D strip test: 0.2 	coating 	Cu: no change; Ag: no change; Pb: voluminous white corrosion, heterogeneous 	
Benjamin Moore M42 platinum gray epoxy on mylar 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2005/08/12 	NMAI 	Oddy Test 	 	noticeable odor on opening jar 	coating 	Cu: no change; Ag: no change; Pb: darkened 	
Benjamin Moore M42 clear epoxy on Sintra 	Benjamin Moore 	 	pass 	2005/07/27 	NMAI 	Oddy Test 	 	retest: Pb coupons reacted differently, A-D strip test: no change 	coating 	Cu: shiny; Ag: shiny; Pb: darkened 	
Benjamin Moore M42 clear epoxy on Sintra 	Benjamin Moore 	 	pass 	2005/07/27 	NMAI 	Oddy Test 	 	retest: Pb coupons reacted differently, A-D strip test: no change 	coating 	Cu: shiny; Ag: shiny; Pb: heterogeneous scattered white crystals - condensation? 	
BM Stays Clear 423 acrylic on Appleply 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2005/03/10 	NMAI 	Oddy Test 	 	A-D strip test: level 1 	coating 	Cu: no change; Ag: no change; Pb: overall layer yellow-white corrosion, flakes off easily 	
BM Stays Clear 423 acrylic on Appleply 	Benjamin Moore www.benjaminmoore.com 	 	fail 	2005/03/10 	NMAI 	Oddy Test 	 	 	coating 	 	
Krylon All Purpose Primer Gray 1318 	Krylon www.kpg-industrial.com 	 	Fail 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; Ag: shiny; Pb: overall Cu color, orangy or red, esp along edges; white corr from condens 	
Krylon All Purpose Primer Gray 1318 	Krylon www.kpg-industrial.com 	 	Fail 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; black corrosion outer end from condens; Ag: shiny; Pb: overall Cu color, orangy or red, esp along edges 	
Krylon Crystal Clear 1301 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 7 days 	Coating 	Cu: shiny; slight violet tinge; Ag: shiny; Pb: slightly dark gray 	
Krylon Crystal Clear 1301 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 7 days 	Coating 	Cu: shiny; slight violet tinge; Ag: shiny; Pb: slightly dark gray 	
Krylon Satin Touch Ivory 3510 	Sherwin Williams Co., Krylon Products Group, 800 832 2541 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; Ag: shiny; Pb: slightly dark gray 	
Krylon Satin Touch Ivory 3510 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; slight violet tinge; Ag: shiny; Pb: slightly dark gray; spots of white corrosion from condensation 	
Krylon Ultra Flat Black 1602 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; Ag: shiny; Pb: slightly dark gray 	
Krylon Ultra Flat Black 1602 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; Ag: shiny; Pb: slightly dark gray 	
Krylon UV Resistant Clear Acrylic Spray 1305 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: Slight darker, green tinge; shiny; evidence of condensation probs; Ag: shiny; Pb: slightly dark gray 	
Krylon UV Resistant Clear Acrylic Spray 1305 	Krylon www.kpg-industrial.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; spots of black corr from condens; violet tinge outer end; Ag: shiny; Pb: slightly dark gray; white corr from condens 	
Rustoleum Chrome 7718 	Rust-Oleum Corp., www.rustoleum.com 	 	Fail 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; Ag: slight yellow tinge overall; Pb: slightly dark gray 	
Rustoleum Chrome 7718 	Rust-Oleum Corp., www.rustoleum.com 	 	Fail 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; slight violet tinge; Ag: slight yellow tinge overall; Pb: slightly dark gray 	
Rustoleum Gold 7710 	Rust-Oleum Corp., www.rustoleum.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; slight violet tinge; Ag: shiny; Pb: slightly dark gray 	
Rustoleum Gold 7710 	Rust-Oleum Corp., www.rustoleum.com 	 	Pass 	2004/02/27 	NMAI 	Oddy Test 	 	Samples left in oven 2.5 weeks longer than usual; samples offgas for 4 weeks 	Coating 	Cu: shiny; slight violet tinge; Ag: shiny; Pb: slightly dark gray 	
Agateen Lacquer No.27 on glass slide cover 	Agate Lacquer Mfg.Co. www.agatelacquer.com 	 	Pass 	2003/09/30 	NMAI 	Oddy Test 	 	Allowed to offgas 7 days under fume hood before test 	coating 	Cu: Violet discoloration; significantly more darkened on underside of coupon, but still has some shine; Ag: Shiny - ok; Pb: slightly darkened 	
Agateen Lacquer No.27 on glass slide cover 	Agate Lacquer Mfg.Co. www.agatelacquer.com 	 	Pass 	2003/09/30 	NMAI 	Oddy Test 	 	Allowed to offgas 7 days under fume hood before test 	coating 	Cu: Violet discoloration; still shiny; Ag: Shiny - ok; Pb: slightly darkened 	
B.M. Regal Eggshell Finish 100% Acrylic paint, N310 Ultra Base #1238; , painted on mylar 	www.benjaminmoore.com 	 	pass 	2007/08/06 	NMAI 	Oddy Test 	 	approved without testing 6/4/07 because time limitations and 100% acrylic. Tested after used for case interiors, passed, A-D strip test pass 	coating/paint 	Cu: no change; Ag: no change; Pb: dull, darkened, white, sparkly residue on half of the interior facing surface and on small corner of exterior 	
B.M. Regal Eggshell Finish 100% Acrylic Paint, N319 4B Ultra Base #HC-133; painted on mylar 	www.benjaminmoore.com 	 	pass 	2007/08/06 	NMAI 	Oddy Test 	 	approved without testing 6/4/07 because time limitations and 100% acrylic. Tested after used for case interiors, passed, A-D strip test pass 	coating/paint 	Cu: no change; Ag: no change; Pb: dull, darkened 	
B.M. Regal Eggshell Finish 100% Acrylic Paint, N319 4B Ultra Base #HC-133; painted on mylar 	www.benjaminmoore.com 	 	pass 	2007/08/06 	NMAI 	Oddy Test 	 	approved without testing 6/4/07 because time limitations and 100% acrylic. Tested after used for case interiors, passed, A-D strip test pass 	coating/paint 	Cu: no change; Ag: no change; Pb: dull, darkened 	
Opaci-coat 300 	ICD Coatings; http://www.icdcoatings.com/ 	 	pass 	2007/04/27 	NMAI 	Oddy Test 	 	photo on file 	coating 	Cu: dulled, darkened crimson/brown; Ag: no change; Pb: dulled, slightly darkened 	
Opaci-coat 300 	ICD Coatings; http://www.icdcoatings.com/ 	 	pass 	2007/04/27 	NMAI 	Oddy Test 	 	photo on file 	coating 	Cu: dulled, darkened crimson/brown; Ag: no change; Pb: dulled, slightly darkened 	
1- BM M42 epoxy clear on Appleply; 2- M42 platinum grey 	Benjamin Moore; Sancure:Noveon; Appleply:States Industries 	 	fail 	2007/02/08 	NMAI 	Oddy Test 	 	 	coating 	Cu: dull, considerably darkened; Ag: no change; Pb: slightly darkened 	
1- BM M42 epoxy clear on Appleply; 2- M42 platinum grey 	Benjamin Moore; Sancure:Noveon; Appleply:States Industries 	 	fail 	2007/02/08 	NMAI 	Oddy Test 	 	 	coating 	Cu: dull, considerably darkened; Ag: no change; Pb: 1/3 of coupon completely disintegrated into white powdery corrosion, rest of coupon covered with white corrosion 	
Ben. Moore Platinum Epoxy M42 covered with BM Vapor Barrier 260 on Appleply 	Benjamin Moore; Appleply:States Industries 	 	fail 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: dull orange brown; Ag: no change; Pb: thick white corrosion all over 	
Ben. Moore Platinum Epoxy M42 covered with BM Vapor Barrier 261 on Appleply 	Benjamin Moore; Appleply:States Industries 	 	fail 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: dull orange brown; Ag: no change; Pb: thick white corrosion all over; some yellow crystals 	
Sancure 878 covered with BM Vapor Barrier 260 on Appleply 	Benjamin Moore; Sancure:Noveon; Appleply:States Industries 	 	fail 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: bright metallic orange; Ag: no change; Pb: white corrosion layer all-over, little build-up 	
Sancure 878 covered with BM Vapor Barrier 261 on Appleply 	Benjamin Moore; Sancure:Noveon; Appleply:States Industries 	 	fail 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: bright metallic orange; Ag: no change; Pb: thick white flaking corrosion with thick yellow-brown build-up on exterior side 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Deep #684 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: dulled, darkened 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Deep #684 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: no change 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Deep #685 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: no change 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Deep #685 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: dulled brown; Ag: no change; Pb: slight blue irridescence 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Deep #712 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: dulled 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Deep #712 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: dulled 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Medium #1644 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: slight blue irridescence 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Medium #1644 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: no change 	
Benjamin Moore Regal Matte Wall Satin Flat Finish 215 Color Preview Base Medium #1671 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2006/03/22 	NMAI 	Oddy Test 	 	 	coating 	Cu: no change; Ag: no change; Pb: darkened 	
Camger I-175-50 clear satin finish on Appleply 	 	 	fail 	2008/05/14 	NMAI 	Oddy Test 	 	product more effective than Ceramic Force as a wood vapor barrier, but both technically fail 	coating (as vapor barrier for wood) 	; Pb: white corrosion 	
Camger I-175-50 clear satin finish on Appleply 	 	 	fail 	2008/05/14 	NMAI 	Oddy Test 	 	product more effective than Ceramic Force as a wood vapor barrier, but both technically fail 	coating (as vapor barrier for wood) 	; Pb: white corrosion 	
Benjamin Moore Stays Clear Low Luster 423 acylic polyurethane 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2008/04/16 	NMAI 	Oddy Test 	 	condensation problems 	coating 	Cu: same as control; Ag: same as control; Pb: same as control 	
Benjamin Moore Stays Clear Low Luster 423 acylic polyurethane 	Benjamin Moore www.benjaminmoore.com 	 	pass 	2008/04/16 	NMAI 	Oddy Test 	 	condensation problems 	coating 	Cu: same as control; Ag: same as control; Pb: same as control 	
Appleply with coating of PolyAspartic IFS-645 and Degadur R71 colorless topcoat (Previously untested sample) 	Innovative Floor Systems/RAM RFQ Supply; 410-354-6400 	 	fail 	2007/08/22 	NMAI 	Oddy Test 	 	Sample previously untested ; had been prepared for original testing. Interior of jar was dry after 3 weeks…DI H20 may not have been initially added, A-D strip test - slight color change - between 0 and 1. 	coating 	Cu: dull and slightly darkened; Ag: no change; Pb: dull, darkened w/ a slight silvery-white powdered appearance on interior facing surface 	
Appleply with coating of PolyAspartic IFS-645 and Degadur R71 colorless topcoat 	Innovative Floor Systems www.innovativefloors.com 	 	fail 	2007/08/22 	NMAI 	Oddy Test 	 	retesting same sample previously tested, A-D strip test: slight color change - between 0 and 1 	coating 	Cu: side facing interior of beaker is considerably darker than control, dull overall; Ag: no change; Pb: white powdery coating over entire surface; thick yellowish white crystals on interior facing surface 	
Appleply with coating of PolyAspartic IFS-645 and Degadur R71 colorless topcoat 	Innovative Floor Systems www.innovativefloors.com 	 	fail 	2007/08/22 	NMAI 	Oddy Test 	 	retesting same sample previously tested, A-D strip test: slight color change - between 0 and 1 	coating 	Cu: side facing interior of beaker is considerably darker than control, dull overall; Ag: no change; Pb: white powdery coating over entire surface; thick yellowish white crystals on interior facing surface 	
B.M. Regal Eggshell Finish 100% Acrylic paint, N310 Ultra Base #1238; , painted on mylar 	www.benjaminmoore.com 	 	pass 	2007/08/06 	NMAI 	Oddy Test 	 	approved without testing 6/4/07 because time limitations and 100% acrylic. Tested after used for case interiors, passed, A-D strip test pass 	coating/paint 	Cu: no change; Ag: no change; Pb: dull, darkened 	
Aquapon 98-1 over appleply 	by PPG Industries, Inc 	 	fail 	2014/05/13 	NMAI 	Oddy Test 	 	 	epoxy paint 	Cu: uneven purplish/multi-colored oxidation; Ag: very slight grey corrosion; Pb: overall white crystalline corrosion, built up on edges and thickest at bottom 	
WB Urethane Sealer 	Terrazzo & Marble Companies 	Terrazzo & Marble Companies 	Temporary 	2021/06/10 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Clear, water-based, non-yellowing sealer with stain and chemical resistance for Terroxy flooring systems; 48-72 hour full cure; pH range 7-10 Purchased April 2021, poured onto mylar to cure for 6 days before testing 	 	-Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish)	 	
Terroxy Resin Systems-Terrazzo Primer Part A and B 	Terrazzo and Marble Companies 	Terrazzo and Marble Companies 	Temporary 	2021/04/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two part epoxy primer designed for concrete, wood, and masonry surface application; 24 hour cure time, 2 part A to 1 part B by volume; Part A contains Epoxy resin, nonylphenol, clycicyl ether, benzyl alcohol, Part B contains nonylphenol, formaldehyde plymer with benzeneamine hydrogenated, benzyl alcohol, tetraethylenepentamine (TEPA), Tris-2,4,6 (dimethylaminomethyl)phenol; combined 40 mL part A with 20 mL part B in a plastic cup, then spread on mylar and allowed to cure for 3 days; Purchased March 2021 	 	-Coating - Floor (eg.: anti-wear, anti-slip) 	 	
Terroxy Resin Systems Matrix Part A and B 	Terrazzo and Marble Companies 	Terrazzo and Marble Companies 	Fail 	2021/04/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Pigmented two part epoxy for terrazzo flooring systems, part A tinted grey by manufacturer; 18-24 hour cure time, 5:1 parts A and B by volume; part A contains Epoxy resin, calcium carbonate, titanium dioxide, crystalline silica, silicon dioxide, methyl ester, glycicyl ether, part B contains 4-Nonylphenol, triethylenetetramine, diaminopolypropylene glycol, (2-aminoethyl)ethanolamine, aminoethylpiperazine, diethylenetriamine, tetraethylenepentamine; combined 25 mL part A and 5 mL part B in a plastic cup, then spread on mylar and cured for 3 days; Purchased March 2021 	 	-Coating - Floor (eg.: anti-wear, anti-slip) 	 	
Terroxy Resin Systems, Terrazzo WB Acrylic Sealer + 	Terrazzo and Marble Companies 	Terrazzo and Marble Companies 	Fail 	2021/04/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Thin, single part floor finish that combines deep gloss and high durability; 36-48 hour cure time; contains 2-(2-ethoxyethoxy)ethanol and tris(2-butoxyethyl)phosphate; cured on mylar for 3 days; Purchased March 2021 	 	-Coating - Floor (eg.: anti-wear, anti-slip) 	 	
ISO-Crack Epoxy Membrane Part A and B 	Terrazzo and Marble Companies 	Terrazzo and Marble Companies 	Temporary 	2021/04/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Two part epoxy floor coating designed to suppress reflective cracking in Terroxy Resin flooring systems; 24 hour full cure, 1:1 part A and B by volume; contains epoxy resin, calcium carbonate, glycidyl ether, silicon dioxide, titanium dioxide, crystalline silica; Prepared by combining 20 mL each part in a plastic cup and mixed until homogenous, then spread on mylar and cured for 3 days; Received March 2021 	 	-Coating - Floor (eg.: anti-wear, anti-slip) 	 	
Plasti-Dip Black Multi-Purpose Rubber Coating 	Plasti Dip International 	Auto Zone 	FAIL 	2020/12/02 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Matte black synthetic rubber coating applied by spraying, brushing, or dipping; Resists moisture, acids, abrasion, corrosion, slipping; 30 minutes dry between coats, 4 hours per coat to full dry; 4 coats sprayed onto mylar, allowed to cure for 2 days prior to testing, removed from mylar before testing; Purchased in 2020 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Monokote MK-6 HY Cementitious Fireproofing 	GCP Applied Technologies 	GCP Applied Technologies 	Temporary 	2020/11/04 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Single component, spray applied, mill-mixed fire resistive plaster; Contains calcium carbonate, quartz (SiO2), and calcium sulfate; Sample prepared by manufacturer, received September 2020 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Monokote Z-146 High Density Proofing 	GCP Applied Technologies 	GCP Applied Technologies 	Temporary 	2020/11/04 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Portland cement-based, factory-mixed high density fireproofing; applied with water and spray applied directly to structural steel; provides up to 4 hours of fire resistance; 40 pcf dry density; contains portland cement, quarts (SiO2), and hexavalent chromium; sample prepared by manufacturer, received September 2020 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Bonaseal waterborne organic solvent sealer (now known as ClassicSeal) 	Bona 	Amazon 	FAIL 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Wood floor sealer specially formulated for use with Bona Naturalem Bona Traffic, and Bona Mega Finishes. Non-yellowing, odorless, 2-3 hr dry time, maximum cure: 1 week. pH 7.8, 1.04 specific gravity. Contains water, acrylic resin, (2-methoxymethylethoxy)propanol (also known as dipropylene glycol monomethyl ether), and defoamers. Purchased August 2020, cured for 20 days 	 	Coating - Floor (eg.: anti-wear, anti-slip) 	 	
BonaTraffic HD (+ hardener) waterborne floor finish 	Bona 	Amazon 	Temporary 	2020/10/21 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Clear, colorless, nonflammable finishing for hardwood floor. Dries in about 2-3 hours, full cure in 3 days. pH 7.9, 1.04 specific gravity, 0°C melting point, 100°C boiling point. Contains water, polymeric resins, and amorphous silica. Hardner has 1.09 relative density, contains propylene carbonate, hydrofilic aliphatic polyisocyanate, and Hexane, 1,6-diisocyanato-, homopolymer. Purchased August 2020, cured for 20 days 	 	Coating - Floor (eg.: anti-wear, anti-slip) 	 	
DC315, intumescent paint 	International Fireproof Technology, Inc. 	International Fireproof Technology, Inc. 	FAIL 	2020/10/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Intumescent fireproofing paint, contains ammonium polyphosphate, melamine, pentaerythritol, PVAC resin, and titanium dioxide. Received January 2020, cured for 7 days 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Sancure™ 878, polyurethane sealant 	Lubrizol 	Lubrizol 	Temporary 	2020/09/29 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	High gloss polyurethane sealant for hardness, abrasion resistance and flexibility; co-solvent free. Adhesion to wood, plastic, metal, and textiles. Received February 2020, cured for 5 days 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
394 Perimeprime, anti-corrosion primer 	Tnemec 	Tnemec 	FAIL 	2020/09/18 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Anti-corrosion primer for use under fireproofing systems. Specially formulated, one-component, moisture-cured, micaceous iron oxide and zinc filled primer that offers superior bonding to marginally prepared rusty steel and tightly adhered old coatings. Triple barrier mechanism of zinc, mio and urethane resin built into the dry film. 100°C boiling point, 2.56 specific gravity. Contains micaceous iron oxide, zinc (total dust), diphenylmethane diisocyanate polymer, p-chlorobenzotrifluoride, aromatic hydrocarbon mixture, 1,2,4-trimethylbenzene, C.I. pigment brown 24, tert-butyl acetate, diphenylmethane diisocyanate reactive monomer, talc (respirable dust), polymeric MDI, p-toluenesulfonyl isocyanate, 1,3,5-trimethylbenzene, diphenylmethane-2,2-diisocyanate monomer, and cumene (skin). Received August 2020, cured onto steel panels by manufacturer	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
27WB Typoxy 	Tnemec 	Tnemec 	Temporary 	2020/09/18 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	A unique, low odor, low VOC, water-based epoxy coating fordurability and corrosion resistance on steel and concrete structures. 72°C boiling point, 1.59 specific gravity. Contains titanium oxide (total dust), epoxyamine adduct resin, amorphous calcium aluminosilicate, silicon dioxide/aluminum oxides, crystalline silica (quartz), amorphous silica, proprietary pigment, and boron oxide. Received August 2020, cured onto steel panels by manufacturer 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Cafco Blaze Shield II 	Isolatek International 	Isolatek International 	FAIL 	2020/09/04 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	A high strength commercial density, Portland cement based Spray-Applied Fire Resistive Material (SFRM). R-value of 2.94 R/inch, 0.240 g/mL density. Contains slag wool, Portland cement, quartz (SiO2), and petroleum distillates, hydrotreated middle. Received July 2020 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Southwest Type 7HD Fireproofing 	Carboline 	Carboline 	Temporary 	2020/03/04 	MMA 	Oddy Test (method: 20190226_OT_1) 	A cementitious spray-applied fire-resistive materials intended for the fire protection of structural columns, beams, joists, decks, walls, roofs, girders, floors and pre-cast concrete units. 40 lb./ft³ (640 kg/m³) average density. ~1-inch thick sample received January 2020. Sprayed onto wooden board during preparation according to manufacturer, but came without the board. 	Color: Grey 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Pyrocrete 40 Fireproofing 	Carboline 	Carboline 	Temporary 	2020/03/04 	MMA 	Oddy Test (method: 20190226_OT_1) 	Portland cement based, cementitious fireproofing. Provides both hydrocarbon and cellulosic fire protection for structural steel. Can also be used to upgrade the fire resistance of existing concrete. 40 lb./ft³ (640 kg/m³) density. ~1-inch thick sample received January 2020. Sprayed onto wooden board during preparation according to manufacturer, but came without the board 	Color: Tan 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Krylon Color Master, gloss crystal clear spray paint,3403 	Rust-Oleum Corp. 	Walmart 	Permanent 	2019/01/11 	FMNH 	Oddy Test 	Gloss crystal clear spray. Acetone, n-butyl acetate, propane, butane, ethyl 3-ethoxypropionate, xylene (mixed isomers), ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Krylon Color Master, flat crystal clear spray paint,3430 	Rust-Oleum Corp. 	Walmart 	Permanent 	2019/01/11 	FMNH 	Oddy Test 	Flat crystal clear spray. Acetone, n-butyl acetate, propane, butane, xylene (mixed isomers), ethyl 3-ethoxypropionate, amorphous silica, ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Krylon Industrial Tough Coat Primer, light-gray spray paint,A00341007 	Sherwin-Williams Company 	Global Industrial 	Permanent 	2019/01/11 	FMNH 	Oddy Test 	Light-gray primer. Acetone, Propane, Butane, Xylene, Isobutyl Acetate, Toluene, 2-Propanol, Titanium Dioxide, Ethybenzene, Dibutly phthalate. 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Rust-Oleum 2X Ultra Cover, clear gloss spray paint, 327864 	Rust-Oleum Corp. 	Walmart 	Permanent 	2019/01/11 	FMNH 	Oddy Test 	Clear gloss spray. Acetone, n-butyl acetate, propane, n-butane, 1-methoxy-2-propyl acetate, ethyl 3-ethoxypropionate, xylenes, ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Rust-Oleum 2x Ultra Cover, matte clear spray paint, 327862 	Rust-Oleum Corp. 	Walmart 	Permanent 	2019/01/11 	FMNH 	Oddy Test 	Clear matte spray. Acetone, n-butyl acetate, propane, n-butane, dimethyl carbonate, propylene glycol monobutyl ether, naphta, ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Rust-Oleum Hard Hat High Performance Enamel Primer spray paint, flat grey primer, V2182838 Bar Code 20066 00129 	Rust-Oleum Corp. 	 	Temporary/Limited Use 	2019/08/07 	FMNH 	Oddy Test 	Flat grey primer. Propane, n-butyl acetate, acetone, dimethyl carbonate, hydrous magnesium silicate, n-butane, titanium dioxide, hydrotreated light distillate, solvent naphtha, 1,2,4-trimethylbenzene, zinc phosphate, zinc oxide, methyl ethyl ketoxime, ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Minimal white crystal growth and gray/orange oxidative layer
Silver: Consistent with Control 	
Krylon Colormaster Paint+Primer, indoor/outdoor spray paint, flat white, 3432 	Krylon Products Group 	Walmart 	Fail, Unsuitable 	2018/03/30 	FMNH 	Oddy Test 	Flat white primer. Acetone, propane, n-butyl acetate, butane, aliphatic hydrocarbon solvent, ethyl 3-ethoxpropionate, xylene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystal growth overall
Silver: Consistent with Control 	
Krylon Colormaster Primer indoor/outdoor spray paint, flat white, 3455 	Krylon Products Group 	Walmart 	Fail, Unsuitable 	2018/03/30 	FMNH 	Oddy Test 	Flat white primer. Acetone, propane, ethylbenzene, dimethyl carbonate, butane, 2-methyl-1-propanol, aliphatic hydrocarbon solvent 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystal growth overall
Silver: Consistent with Control 	
Krylon Plastic Primer indoor/outdoor spray paint, white, 51321 	Krylon Products Group 	Walmart 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Flat white primer 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystal growth overall
Silver: Consistent with Control 	
Rust-Oleum Painters Touch 2X Ultra Cover primer spray paint, flat white, 249058 	Rust-Oleum Corp. 	Menards 	Fail, Unsuitable 	2018/03/30 	FMNH 	Oddy Test 	Flat white spray paint. Acetone, petroleum distillates, and xylene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystal growth overall
Silver: Consistent with Control 	
Krylon Industrial Acryli-Quik Primer spray paint, black, 1316, #38EM22 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2017/05/08 	FMNH 	Oddy Test 	Black acrylic lacquer. Acetone, toluene, propane, butane, light aliphatic hydrocarbon solven, 2-methyl-1-propanol 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Heavy white crystals 
Silver: Consistent with Control 	
Krylon Industrial Acryli-Quik Primer spray paint, reddish brown, 1317, #38EM46 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Brown acrylic lacquer. Acetone, toluene, propane, butane, light aliphatic hydrocarbon solven, 2-methyl-1-propanol 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Few white crystals
Silver: Consistent with Control 	
Krylon Industrial Acryli-Quik Primer spray paint, flat platinum grey, 1314, #38EM33 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Flat grey acrylic lacquer. Acetone, propane, ethylbenzene, dimethyl carbonate, butane, talc, 2-methyl-1-propanol, titanium dioxide, light aliphatic hydrocarbon solvent 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Few white crystals
Silver: Consistent with Control 	
Krylon Industrial Acryli-Quik Primer spray paint, gray, 1318, #38EM47 	Sherwin-Williams Company 	Grainger 	Pass, Permanent 	2019/08/07 	FMNH 	Oddy Test 	Gray acrylic lacquer. Acetone, toluene, propane, butane, light aliphatic hydrocarbon solvent, 2-methyl-1-propanol, titanium dioxide 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Krylon Industrial Acryli-Quik Spray Paint, flat white, 1502, # 38EM26 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Flat white acrylic lacquer. Acetone, propane, methyl ethyl ketone, xylene, butane, titanium dioxide, ethylbenzene, toluene, methyl isobutyl ketone 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Yellow and white crystals
Silver: Consistent with Control 	
Krylon Industrial Iron Guard Latex Enamel Spray Paint, flat white, 7910, #3CPV3 	Sherwin-Williams Company 	Grainger 	Pass, Permanent 	2019/08/07 	FMNH 	Oddy Test 	Flat white latex. Titanium dioxide, 2-propanol, 2-butoxyethanol 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Krylon Industrial Iron Guard Spray Paint, flat black, 7911, #3CPV4 	Sherwin-Williams Company 	Grainger 	Pass, Permanent 	2019/08/07 	FMNH 	Oddy Test 	Flat black latex enamel. 2-propanol, 2-(2-butoxyethoxy)-ethanol, carbon black 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Krylon Industrial Iron Guard Spray Paint, satin gray, 7914, #3CPV7 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Satin gray latex enamel. Titanium dioxide, 2-butoxyethanol, 2-propanol, carbon black 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Heavy white crystals 
Silver: Consistent with Control 	
Krylon Rust Protector Enamel Spray Paint, flat brown, 69036 	Sherwin-Williams Company 	McMaster-Carr 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Flat brown spray. Acetone, propane, n-butyl acetate, butane, talc, light aliphatic hydrocarbon solvent, xylene, ethyl 3 ethoxypropionate, iron oxide, ethylbenzene, unsaturated fatty acids, carbon black 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Heavy white crystals 
Silver: Consistent with Control 	
Krylon Rust Protector Rust Preventative Primer Spray Paint, gloss gray, 69038, # 38EP15 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Gloss gray spray. Acetone, propane, ethylbenzene, dimethyl carbonate, butane, talc, 2-methyl-1-propanol, titanium dioxide, light aliphatic hydrocarbon solvent 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Few white crystals 
Silver: Consistent with Control 	
Krylon Supermaxx All-In-One Spray Paint and Primer, flat black, 8970, #38EN09 	Sherwin-Williams Company 	Grainger 	Fail, Unsuitable 	2019/08/07 	FMNH 	Oddy Test 	Flat black spray. Acetone, propane, n-butyl acetate, butane, talc, aliphatic hydrocarbon solvent, ehyl 3-Eehoxypropionate, xylene, carbon black, ethylbenzene, unsaturated fatty acids 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Heavy white crystals 
Silver: Consistent with Control 	
Plasti-Kote Premium Enamel, flat black, T-2 	The Valspar Corporation 	McMaster-Carr 	Pass, Permanent 	2017/05/08 	FMNH 	Oddy Test 	Flat black enamel. Acetone, methyl isobutyl ketone, butyl acetate, ethyl 3-ethoxypropinate 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Plasti-Kote Premium Primer, gray, T-18 	The Valspar Corporation 	McMaster-Carr 	Fail, Unsuitable 	2017/05/08 	FMNH 	Oddy Test 	Gray primer. Acetone, propane, isobutyl acetate, titanium dioxide, petroleum distillates 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystals 
Silver: Consistent with Control 	
Rust-Oleum High Performance Enamel Primer Spray Paint, flat grey, V2182838 	Rust-Oleum Corp. 	 	Pass, Permanent 	2018/01/16 	FMNH 	Oddy Test 	Flat grey enamel spray. Propane, n-butyl acetate, acetone, dimethyl carbonate, hydrous magnesium silicate, titanium dioxide, n-Butane, hydrotreated light distillate, solvent naphtha, 1,2,4-trimethylbenzene, zinc phosphate, methyl ethyl ketoxime, ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Rust-Oleum High Performance Enamel Spray Paint, flat black, V2178838 	Rust-Oleum Corp. 	 	Fail, Unsuitable 	2018/01/16 	FMNH 	Oddy Test 	Flat black enamel spray. Acetone, propane, hydrous magnesium silicate, n-butyl acetate, n-butane, solvent naphtha, light aromatic hydrotreated, Llght distillate, dimethyl carbonate, 1,2,4-trimethylbenzene, carbon black, ethylbenzene 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Heavy white crystals 
Silver: Consistent with Control 	
Rust-Oleum Industrial Choice Multi-Purpose Spray Paint, flat white, 1690830, #6KP29 	Rust-Oleum Corp. 	Grainger 	Fail, Unsuitable 	2018/01/16 	FMNH 	Oddy Test 	Flat white enamel spray. Acetone, propane, n-butane, titanium dioxide, hydrotreated light distillate, xylenes, hydrous magnesium silicate, naphtha, petroleum, hydrotreated light kaolin, ethylbenzene, methyl ethyl ketoxime 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystsals
Silver: Consistent with Control 	
Rust-Oleum Industrial Choice Multi-Purpose Primer, gray, 1680830, #6KP23 	Rust-Oleum Corp. 	Grainger 	Fail, Unsuitable 	2017/05/08 	FMNH 	Oddy Test 	Gray primer. Acetone, propane, titanium dioxide, n-butane, naphtha, light hydrotreated distillate, hydrous magnesium silicate, n-butyl acetate, xylenes, zinc phosphate, ethylbenzene, carbon black, octane, zinc oxide 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystals
Silver: Consistent with Control 	
Duralaq Waterborne Finish, 1 WB.104 	Benjamin Moore 	 	Pass, Permanent 	2016/09/13 	FMNH 	Oddy Test 	Waterborne paint. Propylene glycol, propylene glycol monoethyl ether, 2-butoxyethanol, solvent naptha 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, black, 229S1 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Carbon black, wollanstonite 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, bright blue, 229B1 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/10/25 	FMNH 	Oddy Test 	Colorant. Proprietary pigment, wollanstonite, alcohols 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, gray, 229S2 	Benjamin Moore 	JC Licht 	Fail, Unsuitable 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Kaolin, carbon black 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, magenta, 229M1 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Kaolin 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, orange, 229O1 	Benjamin Moore 	JC Licht 	Fail, Unsuitable 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Zinc oxide 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystals
Silver: Consistent with Control 	
Gennex Waterborne Colorant, organic red, 229R2 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/10/25 	FMNH 	Oddy Test 	Colorant. Wollanstonite 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, organic yellow, 229Y1 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/12/21 	FMNH 	Oddy Test 	Colorant 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, organic yellow, 229Y2 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/12/21 	FMNH 	Oddy Test 	Colorant 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystals
Silver: Consistent with Control 	
Gennex Waterborne Colorant, oxide red, 229R3 	Benjamin Moore 	JC Licht 	Fail, Unsuitable 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Iron oxide 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, oxide yellow, 229Y3 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/10/25 	FMNH 	Oddy Test 	Colorant 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Gennex Waterborne Colorant, red toner, 229R1 	Benjamin Moore 	JC Licht 	Fail, Unsuitable 	2016/10/25 	FMNH 	Oddy Test 	Colorant. Kaolin 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Yellow crystals
Silver: Consistent with Control 	
Gennex Waterborne Colorant, thalo green, 229G1 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Proprietary pigment, kaolin 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: White crystals
Silver: Consistent with Control 	
Gennex Waterborne Colorant, white 229W1 	Benjamin Moore 	JC Licht 	Pass, Permanent 	2016/12/21 	FMNH 	Oddy Test 	Colorant. Titanium dioxide, amorphous silica, aluminum hydroxide 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Ben Waterborne Interior Flat Finish Base 1, W6251X, tinted to #2060-30 (seaport blue) 	Benjamin Moore 	Thybony Paint 	Pass, Permanent 	2015/10/14 	FMNH 	Oddy Test 	Water-thinned paint. Titanium dioxide, kaolin, amorphous silica 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Ben Flat Premium Interior Paint & Primer, W625-1X, tinted to SICO paint #6198-21 (very pale grey) 	Benjamin Moore 	Thybony Paint 	Pass, Permanent 	2015/10/14 	FMNH 	Oddy Test 	Water-thinned paint. Titanium dioxide, kaolin, amorphous silica 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Natura Flat Waterborne Interior Paint and Primer, Premium Performance, 512-1X, tinted to SICO paint #6198-21 (very pale grey)	Benjamin Moore 	Thybony Paint 	Pass, Permanent 	2015/09/30 	FMNH 	Oddy Test 	Acrylic waterborne paint. Titanium dioxide, nepheline syenite, calcined kaolin, amorphous silica, diatomaceous earth 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Natura Interior Waterborne Paint, flat, 512, tinted to #2060-30 (seaport blue) 	Benjamin Moore 	Thybony Paint 	Pass, Permanent 	2015/10/14 	FMNH 	Oddy Test 	Acrylic waterborne paint. Titanium dioxide, nepheline syenite, calcined kaolin, amorphous silica 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
Natura Waterborne Interior Paint, eggshell finish, 5131X tinted to #2060-30 (seaport blue) 	Benjamin Moore 	Thybony Paint 	Pass, Permanent 	2015/10/14 	FMNH 	Oddy Test 	Acrylic waterborne paint. Titanium dioxide, nepheline syenite, calcined kaolin, amorphous silica 	 	Coating - paint & primer 	Copper: Consistent with Control
Lead: Consistent with Control
Silver: Consistent with Control 	
OECE 414-9001 / White Back Paint for Glass 	OECE [Organizzazione Economica Commercio Emiliano (Emilia Commerce Economic Organization)] 	 	Pass, Permanent 	2016/08/04 	BKM 	Oddy Test 	White back paint for glass - case material for Goppion cases 	Cu corrosion appeared the same as on both controls 	Coating - paint & primer 	Pb: No corrosion; 
Cu: very minor darkening; 
Ag: good - no corrosion 	
EuroPolveri RAL 9005 / Powdercoat (Textured) on Steel 	EuroPolveri 	 	Pass, Permanent 	2016/08/04 	BKM 	Oddy Test 	Powdercoated steel 	Cu corrosion appeared the same as on both controls 	Coating - paint & primer 	Pb: No corrosion; 
Cu: very minor darkening; 
Ag: no corrosion 	
Dow Corning 3145 RTV MIL-A-46146 Transparent / Structural Sealant and Adhesive 	Dow Corning 	 	Pass, Permanent 	2016/09/21 	BKM 	Oddy Test 	Sealant and Adhesive 	Cu corrosion appeared the same as on both controls 	Polymer - adhesive caulk 	Pb: No corrosion; 
Cu: very minor darkening; 
Ag: no corrosion 	
Dow Corning 7091 Black / Structural Adhesive / Sealant 	Dow Corning 	 	Pass, Permanent 	2016/09/21 	BKM 	Oddy Test 	Sealant and Adhesive 	Cu corrosion appeared the same as on both controls 	Polymer - adhesive caulk 	Pb: No corrosion; 
Cu: minor darkening; 
Ag: no corrosion 	
Dow Corning 3145 RTV MIL-A-46146 Transparent / Structural Sealant and Adhesive 	Dow Corning 	 	Pass, Permanent 	2017/05/26 	BKM 	Oddy Test 	Silicone adhesive 	same as controls 	Polymer - adhesive caulk 	Pb: dark gray, same as control; 
Cu: red - same as control; 
Ag: no corrosion 	
Dow Corning RTV Sealant 737 Neutral Cure Sealant 	Dow Corning 	 	Fail, Unsuitable 	2017/05/26 	BKM 	Oddy Test 	Silicone adhesive 	much more corrosion on Pb than control 	Polymer - adhesive caulk 	Pb: white corrosion, none on control; 
Cu: red - same as control; 
Ag: no corrosion 	
DOW Corning RTV sealant 737 Neutral Cure Sealant, 100% silicone rubber 	Dow Corning 	 	Fail, Unsuitable 	2018/10/05 	BKM 	Oddy Test 	sealing casework (SmallCorp cases on the 2nd floor) 	extended Oddy test - 52 days 	Polymer - adhesive caulk 	Pb: significantly darker than controls; 
Cu: multicolored corrosion; 
Ag: no corrosion 	
DOW Corning RTV sealant 737 Neutral Cure Sealant, 100% silicone rubber 	Dow Corning 	 	Pass, Permanent 	2018/12/17 	BKM 	Oddy Test 	sealing casework (SmallCorp cases on the 2nd floor) 	 	Polymer - adhesive caulk 	Pb: no corrosion; 
Cu: darkened slightly compared to control; 
Ag: no corrosion 	
OECE 414-9001 / White Back Paint for Glass + Dow Corning 7091 Black / Structural Adhesive / Sealant 	OECE [Organizzazione Economica Commercio Emiliano (Emilia Commerce Economic Organization)] and Dow Corning	 	Pass, Permanent 	2016/09/21 	BKM 	Oddy Test 	2 Materials: Glass tested in combination w/ Adhesive 	Cu corrosion appeared the same as on both controls 	Coating - paint & primer 	Pb: No corrosion; 
Cu: slightly red, but okay; 
Ag: no corrosion 	
CAFCO® 300 	Isolatek International 	Isolatek International 	PASS 	2020/01/08 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Wet-mix gypsum based spray-applied fire resistive material; Sprayed and prepared onto wooden board by manufacturer to a thickness of less than 1 inch, tested without wood, test sample taken from area farthest from the board; Mix time of 2 minutes, mixed material must be used within 30 minutes, set-in time of 4-7 hours; A minimum substrate temperature: 40°F; Acquired November 2019 	Color: Beige 	Coating - protective (eg.: anti-UV, anti-abraision, anti-tarnish)	 	
Nazdar 4700 Series Water-based Screen Ink (4724) (formerly Aquasafe 2700 series) 	Nazdar Ink Technologies 	 	Unsuitable 	2019/03/25 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Permanent acrylic ink - Brown - Brushed on Mylar; air dried for 4 weeks; cut to weight; tested on Mylar 	AMNH Test #34 	Coating - paint or primer 	Copper: heavy haze - Silver: OK - Lead: light white compacted corrosion 	
Speedball Acrylic Screen Printing Ink 	Speed Ball 	 	Temporary 	2019/03/25 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Permanent acrylic ink - Black - Brushed on Mylar; air dried for 4 weeks; cut to weight; tested on Mylar 	AMNH Test #35 	Coating - paint or primer 	Copper: slight red tarnish - Silver: white film - Lead: darkening, light white compacted corrosion 	
Dowsil 7091 Adhesive/Sealant 	Dow Corning 	 	Temporary 	2019/03/25 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	One component neutral curing silicone (alkoxy cure system - condensation cure); Formed-In-Place Gasket (FIPG) material; contains silicone, methanol - Black - Cured on Mylar for 1 week; removed from Mylar and cut to weight 	AMNH Test #36 	Sealant - caulk 	Copper: very slight red tarnish - Silver: - Lead: Darkening, Thin Yellow/green compacted corrosion 	
Dowsil 3145 RTV MIL-A-46146 Adhesive Sealant Clear 	Dow Corning 	 	Temporary 	2019/03/25 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	One-part polydimethylsiloxane adhesive (silicone elastomer); contains methyltrimethoxysilane, methanol, octamethyl cyclotetrasiloxane (D4), dimethyldimethoxysilane (DMDEOS) - Clear - Cured on Mylar; removed from Mylar and cut to weight 	AMNH Test #37 	Sealant - caulk 	Copper: OK - Silver: OK - Lead: darkening 	
Nazdar 9700 Series SV Screen Ink (9724) 	Nazdar Ink Technologies 	Color Edge 	Unsuitable 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	High gloss, solvent-based screen ink; contains 2-butoxyethanol - Black - Brushed on Mylar; air dried for 10 days; cut to weight and tested on Mylar. 	AMNH Test #55 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Thick Yellow/green compacted corrosion, Fluffy white crystals 	
Nazdar 9700 Series SV Screen Ink 	Nazdar Ink Technologies 	ColorEdge 	Unsuitable 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	High gloss, solvent-based screen ink; contains 2-butoxyethanol - Brown - Brushed on Mylar; air dried for 10 days; cut to weight and tested on Mylar. 	AMNH Test #56 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Thick Yellow/green compacted corrosion, Fluffy white crystals 	
Transfer/ rubdown ink 	 	ColorEdge 	Unsuitable 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Dry ink between two non-stick protective sheets - Black - Ink transfered onto Mylar support; only one jar tested 	AMNH Test #57 	Coating - paint or primer 	Copper: Red tarnish, Diffuse heavy haze - Silver: White film likely manufacturer defect - Lead: Thin Yellow/green compacted corrosion, Fluffy white crystals 	
Transfer/ rubdown ink 	 	ColorEdge 	Unsuitable 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Dry ink between two non-stick protective sheets - Brown - Ink transfered onto Mylar support; only one jar tested 	AMNH Test #58 	Coating - paint or primer 	Copper: Rainbow tarnish, Light haze - Silver: White film likely manufacturer defect - Lead: Thin Yellow/green compacted corrosion, Fluffy white crystals 	
Kodak Ektacolor RA Chemicals on Kodak Professional Endura Premium Paper 	Kodak Alaris 	ColorEdge 	Temporary 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Ektacolor RA Chemicals for Process RA-4 (photographic processing); on Professional Endura Premium Paper (resin-coated multi-layers paper) - White - Cut to weight 	AMNH Test #74 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening, Light yellow tinge overall 	
Epson UltraChrome HDX Ink-jet Inks on Epson Archival Matte Paper 	Epson 	ColorEdge 	Temporary 	2019/05/14 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	UltraChrome HDX Inks for ink-jet process printing; contains water, glycerol, triethanol amine (TEOA); on Archival Matte Pape white paper - Black (T8041), dark blue, and dark brown inks - Cut to weight 	AMNH Test #75 	Coating - paint or primer (ink) 	Copper: OK - Silver: OK - Lead: Coupon B Slight darkening, Coupon A light blue tarnish 	
Natura Waterborne Interior Paint Semi-gloss Finish base 4 (5144X) (2053-20) 	Benjamin Moore 	Beacon Paint 	Temporary 	2019/06/20 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex, zero VOC - Dark teal - Spread on Mylar; air dried for 5 weeks including one week at 45C; cut to weight; tested on Mylar 	AMNH Test #95 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Darkening 	
Natura Waterborne Interior Paint Semi-gloss Finish (1651) 	Benjamin Moore 	Beacon Paint 	Temporary 	2019/06/20 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex, zero VOC - Dark teal - Spread on Mylar; air dried for 5 weeks including one week at 45C; cut to weight; tested on Mylar 	AMNH Test #96 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Slight darkening, Light white compacted corrosion 	
Natura Waterborne Interior Paint Semi-gloss Finish (2057-30) 	Benjamin Moore 	Beacon Paint 	Temporary 	2019/06/20 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex, zero VOC - Naples blue - Spread on Mylar; air dried for 5 weeks including one week at 45C; cut to weight; tested on Mylar 	AMNH Test #97 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: Light purple tarnish - Lead: Darkening 	
Natura Waterborne Interior Paint Semi-gloss Finish (2130-20) 	Benjamin Moore 	Beacon Paint 	Temporary 	2019/06/20 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex, zero VOC - Pine cone brown - Spread on Mylar; air dried for 5 weeks including one week at 45C; cut to weight; tested on Mylar 	AMNH Test #98 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Thin Yellow/green compacted corrosion 	
Aquasafe 2700 series #2775 (now 4700 series) 	Nazdar Ink Technologies 	 	Temporary 	2019/07/10 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Gloss water base screen ink; contains titanium dioxide, dipropylene glycol monmethyl ether, 2-(dimethylamino)ethanol, nonylphenol, additives - Super Opaque White - Spread on Mylar; air dried for 2 weeks; cut to weight and tested on Mylar. 	AMNH Test #164 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: OK - Lead: Very thin Yellow/green compacted corrosion, Slight darkening 	
Aura Waterborne Interior Eggshell Finish Base 1 (5241X) 	Benjamin Moore 	 	Temporary 	2019/07/10 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - White - Spread on Mylar; air dried for 3 weeks; cut to weight and tested on Mylar. 	AMNH Test #165 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Very light white compacted corrosion, Darkening, Thin Yellow/green compacted corrosion 	
Aura Waterborne Interior Eggshell Finish (2057-10) 	Benjamin Moore 	 	Temporary 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - River blue - Spread on Mylar; air dried for 3 weeks; cut to weight and tested on Mylar 	AMNH Test #178 	Coating - paint or primer 	Copper: Slight red tarnish - Silver: Very light purple/pink tarnish - Lead: Violet/pink tarnish, Light white compacted corrosion 	
Ink Jet ink T8041 on LexJet Premium Archival Matte Paper 	Epson 	ColorEdge 	Temporary 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Ink jet inks on LexJet Premium Archival Matte Paper - Blacks, blues - Cut to weight 	AMNH Test #179 	Coating - paint or primer (Ink) 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Canon Lucia inkjet inks (1033B to 1042B and clear cartridge 2442B) on Somerset Enhanced Velvet 225 paper 	Canon, Moab 	Duggal 	Temporary 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Inkjet inks on Somerset Enhanced Velvet 225 paper - All colors including black - Cut to weight 	AMNH Test #180 	Coating - paint or primer (Ink) 	Copper: OK - Silver: Light purple tarnish (coupon B) - Lead: Blue tarnish, Violet tarnish 	
Lucia inkjet inks (1033B-1042B, 2442B) on Entrada Rag Bright 300 	Canon (ink), Moab (paper) 	Duggal 	Temporary 	2019/07/29 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Inkjet inks on Entrada Rag Bright 300 paper - All colors (including black) - Cut to weight 	AMNH Test #181 	Coating - paint or primer (ink) 	Copper: OK - Silver: OK, slight darkening of the edges - Lead: Very slight darkening 	
RAL series Powder Coating (teal) 	NIC Industries (Inc.) 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Powder coating; polyester resin - Teal - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #198 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Thin Yellow/green compacted corrosion on coupon B 	
Aura Waterborne Interior Eggshell Finish (2062-10 ) 	Benjamin Moore 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Dark blue - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #200 	Coating - paint or primer 	Copper: OK - Silver: Very light purple tarnish only near the band, White film likely manufacturer defect - Lead: Light white compacted corrosion heavier at base and edges 	
Aura Waterborne Interior Eggshell Finish (2057-20) 	Benjamin Moore 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Teal - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #201 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Light white compacted corrosion 	
Aura Waterborne Interior Eggshell Finish (1673) 	Benjamin Moore 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Blue/ grey - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #202 	Coating - paint or primer 	Copper: OK - Silver: light purple tarnish on band only - Lead: Darkening, Light white compacted corrosion, Light fluffy white crystals 	
Aura Waterborne Interior Eggshell Finish (1652) 	Benjamin Moore 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Dark teal - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #203 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Darkening, Very light white compacted corrosion 	
Aura Waterborne Interior Eggshell Finish (2134-20) 	Benjamin Moore 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Medium brown - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #204 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Darkening, Very light white compacted corrosion 	
Aura Waterborne Interior Eggshell Finish (2134-30) 	Benjamin Moore 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Grey/brown - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #205 	Coating - paint or primer 	Copper: OK - Silver: Light purple tarnish - Lead: Slight darkening, Thin Yellow/green compacted corrosion, Light white compacted corrosion 	
MAP-LVS: Polyester Primer Surfacer (6001SP) 	Matthews Paint 	 	Unsuitable 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Matthews Acrylic Polyurethane Ultra Low VOC, chemically crossed linked; contains styrene, acrylate monomer - White - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #206 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Thin yellow/ green compacted corrosion on A coupon, Light white compacted corrosion 	
MAP-LVS: Low VOC Satin Paint (MAP-LVS-1) with spray reducer (MAP-LVRS02) with hardener (MAP LVX270) 	Matthews Paint 	 	Unsuitable 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Matthews Acrylic Polyurethane Ultra Low VOC (mixture ratio: 3 paint:1 hardener:1 reducer); reducer contains trifluorotoluene, acetylacetone; hardener contains hexamethylene diisocyanate (HDI), trifluorotoluene; paint contains trifluorotoluene, pyrrolo, heptane-2-one, 2-ethylhexyl acetate, pentane-2-4-dione, 2-butoxyethanol, 2-methoxy-1-methylethyl acetate (PGMEA), UV-328. - Teal - Brushed on Mylar (not air-brushed); air dried for 4 weeks; cut to weight; tested on Mylar. 	AMNH Test #207 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Darkening, Light white compacted corrosion 	
MAP-LVS: Flat clear coat (MAP-LVC238) 	Matthews Paint 	 	Unsuitable 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Matthews Acrylic Polyurethane Ultra Low VOC; contains trifluorotoluene - Clear - Brushed on Mylar; air dried for 4 weeks (blanched upon drying in fumehood); cut to weight; tested on Mylar 	AMNH Test #208 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	Copper: OK - Silver: OK - Lead: Thin orange compacted corrosion on coupon A, Thin Yellow/green compacted corrosion on coupon A, Fluffy white crystals on base of coupon B 	
MAP-LVS: primer, paint, top coat layers 	Matthews Paint 	 	Temporary 	2019/08/23 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Matthews Acrylic Polyurethane Ultra Low VOC (MAP-LVS) layering (primer, paint, top coat); chemically cross linked coating; less than 50g/L VOC - Teal - Layers brushed on Mylar 24hrs apart; top layer blanched; cut to weight and tested on Mylar 	AMNH Test #209 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Aura Waterborne Interior Eggshell Finish (HC 159) 	Benjamin Moore 	 	Temporary 	2019/10/15 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Blue/grey - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #238 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: OK, very slight purple near holder on coupon B - Lead: Rainbow tarnish 	
Aura Waterborne Interior Eggshell Finish (1672) 	Benjamin Moore 	 	Temporary 	2019/10/15 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Light blue grey - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #239 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: Very light purple tarnish - Lead: Rainbow tarnish 	
Aura Waterborne Interior Eggshell Finish (1671) 	Benjamin Moore 	 	Temporary 	2019/10/15 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Light blue - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #240 	Coating - paint or primer 	Copper: OK - Silver: Very light purple tarnish - Lead: Rainbow tarnish, Blue tarnish 	
Colore Powder Coating P.2 series (RAL 230 50 15) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Spruce blue - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #246 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Darkening, Very thin yellow/green compacted corrosion on coupon B 	
Colore Powder Coating P.2 series (RAL 230 40 20) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Loon turquoise - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #247 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening, Very light blue tarnish, Thin yellow/green compacted corrosion 	
Colore Powder Coating P.2 series (RAL 230 20 20) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Prussian blue - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #248 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening, Thin Yellow/green compacted corrosion 	
Colore Powder Coating P.2 series (RAL 220 20 20) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Natural Indigo - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #249 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight blue tarnish 	
Colore Powder Coating P.2 series (RAL 230 30 15) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Berry blue green - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #250 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight blue tarnish on coupon A, Very slight thin yellow/green compacted corrosion on coupon B 	
Colore Powder Coating P.2 series (RAL 240 40 15) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Celeste blue - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #251 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Slight darkening on coupon B, Very slight thin yellow/green compacted corrosion 	
Colore Powder Coating P.2 series (RAL 250 30 15) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Black forest - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #252 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: OK - Lead: violet tarnish on coupon A, very slight thin yellow/green compacted corrosion on coupon B 	
Colore Powder Coating P.2 series (RAL 250 20 20) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Cosmos blue - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #253 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: darkening and very slight thin yellow/green compacted corrosion on coupon B, very slight darkening on coupon A 	
Colore Powder Coating P.2 series (RAL 220 40 20) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Mordant blue - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #254 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very thin Yellow/green compacted corrosion, very slight darkening 	
Colore Powder Coating P.2 series (RAL 220 50 15) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Holbein blue grey - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #255 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: darkening, light blue tarnish, slight thin yellow/green compacted corrosion 	
Colore Powder Coating P.2 series (RAL 220 30 20) 	Colore SRL 	Goppion 	Temporary 	2019/12/02 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Epoxy/polyester hybrid powder coating (heavy metals and TGIC free) - Watercolor Blue - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #256 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: very slight film 	
Accolade Z4680 (Z4600 series - flat) 	Pratt and Lambert Paints 	 	Temporary 	2019/12/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic waterborne paint - Bright White - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #257 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: Very light purple tarnish on edges and along holder - Lead: Darkening, thin yellow/green compacted corrosion 	
Super Spec HP Alkyd Metal Primer P06 (P0601 white) 	Benjamin Moore 	 	Unsuitable 	2019/12/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Modified alkyd with corrosion inhibitors; primer for ferrous substrates - White - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #258 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Fluffy white crystals, Light white compacted corrosion 	
Ultra spec Scuff X Interior Matte Finish (White 4801) 	Benjamin Moore 	 	Temporary 	2019/12/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	One-component latex paint (proprietary acrylic copolymer); contains propanoic acid and anionic surfactant - White - Spread on Mylar; air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #259 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: Light purple tarnish on edges and along holder - Lead: Slight darkening, Thin orange compacted corrosion, light white compacted corrosion 	
Super Spec HP Alkyd Primer and Ultra Spec Scuff-X Paint 	Benjamin Moore 	 	Unsuitable 	2019/12/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Modified alkyd and one-component latex paint - White - Primer spread on Mylar and air dried for 24 hours; paint applied and air dried for 4 weeks; cut to weight and tested on Mylar 	AMNH Test #260 	Coating - paint or primer 	Copper: Very slight red tarnish - Silver: Very ight purple tarnish on coupon A at holder fold - Lead: Fluffy white crystals 	
Interpon D1036 Textura Powder Coating (RAL 8022) 	AkzoNobel 	Goppion 	Temporary 	2019/12/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Polyester powder coating; lead and TGIC free - Black - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #261 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Coupon A: Very slight darkening, darkening on coupon B, very thin yellow/green compacted corrosion 	
Glass Paint Polimat PT-MA02/S (RAL 8019) and CPT-50 hardener 	Materia SRL 	 	Temporary 	2019/12/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Solvent-based acrylic polyurethane glass paint - Brown - Sample B was prepared in lab on Mylar (paint and harderner, ratio 2:1) (mixture was lumpy; air dried for4 weeks; cut to weight and tested on Mylar); Sample A was prepared by supplier (sprayed and cured on glass in Italy) (sample scrapped and tested) 	AMNH Test #264 	Coating - paint or primer 	Copper: OK - Silver: Yellow tarnish on coupon A on lower half, very light blue/blue-green tarnish on coupon B lower edge - Lead: Slight darkening, Fluffy white crystals only on lower half of coupon A 	
Interpon D1036 Textura Powder Coating (RAL 9004) 	AkzoNobel 	Goppion 	Temporary 	2020/01/03 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Polyester powder coating; lead and TGIC free - Black - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #266 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Interpon D1036 Textura Powder Coating (RAL 9005) 	AkzoNobel 	Goppion 	Temporary 	2020/01/03 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Polyester powder coating; lead and TGIC free - Black - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #267 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Interpon D1036 Textura Powder Coating (RAL 9011) 	AkzoNobel 	Goppion 	Temporary 	2020/01/03 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Polyester powder coating; lead and TGIC free - Black - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #268 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Interpon D1036 Textura Powder Coating (RAL 9017) 	AkzoNobel 	Goppion 	Temporary 	2020/01/03 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Polyester powder coating; lead and TGIC free - Black - Sample prepared on aluminum foil by supplier; cut to weight; tested with foil 	AMNH Test #269 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Nazdar 59000 Series Enamel Screen Ink (59122) 	Nazdar 	 	Unsuitable 	2020/01/03 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Glossy solvent-based enamel ink - Flat white - Spread on Mylar; air dried for 3 weeks; cut to weight and tested on Mylar 	AMNH Test #270 	Coating - paint or primer 	Copper: Slight red tarnish - Silver: White film likely manufacturer defect - Lead: Fluffy white crystals 	
Interpon 200 Powder Coating (PZ801I Pu Tra Bonzo "Cerchi Scuri") 	AzkoNobel 	Goppion 	Permanent 	2020/02/19 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Polyurethane-based powder coating - Dark bronze color - Sample prepared by supplier on aluminum panel; scrapped and tested 	AMNH Test #282 	Coating - paint or primer 	Copper: OK - Silver: OK - Lead: Very slight darkening 	
Aura Waterborne Interior Eggshell Finish (2057-20) 	Benjamin Moore 	 	Temporary 	2020/03/13 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Galapagos Turquoise - Spread on Mylar; air dried for 3 weeks; cut to weight and tested on Mylar 	AMNH Test #287 	Coating - paint or primer 	Copper: Slight red tarnish - Silver: Light purple tarnish on edges - Lead: Light white compacted corrosion 	
Aura Waterborne Interior Eggshell Finish (3098) 	Benjamin Moore 	 	Temporary 	2020/03/13 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Medium teal - Spread on Mylar; air dried for 3 weeks; cut to weight and tested on Mylar 	AMNH Test #288 	Coating - paint or primer 	Copper: Slight red tarnish - Silver: Light purple tarnish on the edges - Lead: Light white compacted corrosion 	
Aura Waterborne Interior Eggshell Finish (CSP-690) 	Benjamin Moore 	Beacon Paint 	Temporary 	2020/03/13 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	100% acrylic latex paint; contains hexanedioic acid (adipic acid), sodium C14-C16 olefin sulfonate (anionic surfactant) - Hidden Saphire - Spread on Mylar; air dried for 3 weeks; cut to weight and tested on Mylar 	AMNH Test #289 	Coating - paint or primer 	Copper: Red tarnish - Silver: Very light purple tarnish on the edges - Lead: Light white compacted corrosion 	
Liquitex Professional Spray paint (titanium white) 	Colart 	 	Unsuitable 	2020/03/13 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Water-based technology, no lead, CFCs or aromatic hydrocarbons; contains triethylamine, dimethyl ether, denatured alcohol - Titanium white - Spread on Mylar; air dried for 8 weeks; cut to weight and tested on Mylar 	AMNH Test #292 	Coating - paint or primer 	Copper: Slight red tarnish - Silver: OK - Lead: Fluffy white crystals 	
Enviro-Pox Series 287, epoxy floor coating 	Tnemec Company Inc. 	Tnemec Company Inc. 	PASS 	2019/10/11 	MMA 	Oddy Test (method: 20190226_OT_1 ) 	Waterborne 2 part epoxy-amine adduct; low odor, rapid cure, wear-resistant coating for floors, walls and other substrates; the epoxy was mixed according to the manufacturer's directions and spread in a thin coat onto a BoPET mylar-like sheet using a paint roller 7 days before testing; sample produced September 2019 	Black 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
OECE Paint for case glass, 414-9901 	OECE 	Unknown 	Temporary 	2018/08/01 	MMA 	Oddy Test (method: 20180704_OT ) 	Acrylic/polyurethane blended paint with 1 additive. Spec'd. as 3% by weight '840-03' (additive) and 4% by weight Reticulator 840-02. Dilutable with 0-10% water. Dry for stacking 24-48 hours at 25C (60% RH), 90 min 50C. 150-180 g/m^2; prodced June 2018 	Black 	Coating - paint or primer 	 	
CO-NE65/G 	Materia 	Unknown 	FAIL 	2018/08/01 	MMA 	Oddy Test (method: 20180704_OT ) 	Black acrylic/polyurethane blended paint with adhesion promotor and activator. Spec'd. as (PA-3 + RT-4) 3% and 4% respectively. dilutable at 5-10% with water. Contains opacifiers and organic and inorganic pigments, water and glycol ethers. Produced June 2018 	Black 	Coating - paint or primer 	 	
Resicoat powder coat R4-ES/HGF17R 	Akzo Nobel 	Unknown 	Temporary 	2018/05/31 	MMA 	Oddy Test (method: 20171116_OT ) 	Resin baked onto aluminum; samples were cut to fit into Oddy jar; weight of the aluminum far surpasses 2 grams but was subtracted so that 2 grams of coating was tested; R3-ES - Resicoat electrostatic spray application on preheated surfaces; epoxypowder coating; produced April 2018 	Brown 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
Paintcote Resin, RAL 7012 BPG 	Decorative Resins International LTD 	 	Unsuitable 	2019/02/08 	AMNH 	Oddy Test (method: MMA 20190130_OT) 	Acrylic resin system; Applied to Mylar and allowed to cure - Grey - Peeled/scraped from mylar 	AMNH Test #13 	Coating - paint & primer 	Copper: slight red tarnish (streaks) - Silver: ok - Lead: fluffy white crystals 	
POW 85361-1 Cerchi Chiari 	Akzo Nobel 	Goppion 	Temporary 	2019/02/13 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS	Powder Coating; scraped off of aluminum plate; bronze color; purchased 10/2018; jar A contains: MT100A 20 minutes at 180C on aluminum sheet; jar B contains:MT100A 40 minutes at 180C on aluminum sheet 	Brown, chiari dark 	Coating - paint or primer 	 	
Elast-o-coat (Medium Grey) Resin and Hardener 	Dur-A-Flex 	Dur-A-Flex 	Temporary 	2019/02/13 	MMA 	Oddy Test (method: 20180821_OT ) 	Epoxy flooring; purchased 12/2019; cured for 7 days onto Mylar about 3 mm thick; Details: elast-o-coat resin and Hardener mixed on-site by Scientific Research by volume: 2 resin to 1 hardener. mixed thoroughly for 1 minute. Cure time is 8 hours at 70 degrees F. coat to 10 mil thickness.; Chemical Components: Resin: diglycidyl ether bisphenol A epoxy resin (CAS 25068-38-6) + alkyl phenol blocked polyisocyanate, aliphatic glycidyl ether diluent (oxirane, mono((C12-14-alkyloxy)methyl) derivs.) (CAS 68609-97-2), epoxy resin, titanium dioxide, carbon black, phenol, nonyl-branced. Hardener: benzyl alcohol, salicyclic acid, aminomethyl-3,5,5-trimethylcyclohexylamine, aminoethylethanolamine, 1,3-cyclohexanedimethanamine, aminopropylamorpholine, tris(2,4,6, dimethylaminomethyl) phenol, glyceryl poly(oxypropylene)tramine 	Medium grey 	Coating - Floor (eg.: anti-wear, anti-slip) 	 	
OECE 8019 Paint 	OECE 	Goppion (who sourced from Aurelio Giannobi Industria Specchi)	Temporary 	2018/09/27 	MMA 	Oddy Test (method: 20180821_OT ), SPME GCMS	Details: Painted onto A4 sized glass and scraped off. Equal mixture of paint that went through one heat treatment and paint that went through two heat treatments. One heat treatment equals 40 minutes at 35 degrees Celsius followed by 40 minutes at 70-75 degrees Celsius. The paint formulation is 3 parts 840-03 plus 4 parts 840-02 (activator). 	Brown 	Coating - paint or primer 	 	
737 RTV 	Dow Corning 	 	U 	2016/07/21 	MMA 	Oddy Test (method: 20170623_OT ), SPME GCMS	silicone buildings sealant; Cured for 24 hrs. (per manufacturer) before putting in Oddy test; purchased November 2015 	 	Polymer - adhesive - caulk or sealant 	 	
799 white 	Dow Corning 	 	U 	2016/07/21 	MMA 	Oddy Test (method: 20170623_OT ), SPME GCMS	white silicone buildings sealant; Cured for 14 days (per manufacturer) before putting in Oddy test; purchaed November 2015 	 	Polymer - adhesive - caulk or sealant 	 	
Regal Select Flate Anchor Gray 2126-30 paint (base 547 3X) 	Benjamin Moore 	 	T 	2017/09/11 	MMA 	Oddy Test (method: 20161215_OT ), SPME GCMS	Wall paint; Benjamin Moore Regal Select Flat Anchor Gray 2126-30 paint (base 547 3X); 3 week dry; painted on aluminum foil with brush; Oddy tested on aluminum foil 	 	Coating - paint or primer 	 	
Regal Select Flat Anchor Gray 2126-30 (base 547 3X) 	Benjamin Moore 	 	T 	2017/09/25 	MMA 	Oddy Test (method: 20161215_OT ), SPME GCMS	Paint; 1 week dry; painted on aluminum foil with brush; Oddy tested on aluminum foil 	 	Coating - paint or primer 	 	
Permalac Matte 	Peacock laboratories, Inc., Philly, PA 	Peacock laboratories, Inc. 	Temporary 	2018/03/14 	MMA 	Oddy Test (method: 20171116_OT ) 	Clearcoat laquer; 10554.02 - two coats applied; Chemical Components: toluene and acrylate polymers. Month/Year Purchased: 2/2018 	 	Coating - protective (eg.: anti-UV, anti-abrasion, anti-tarnish) 	 	
9-1374 clear silicone sealant 	Dow Corning 	Dow Corning 	T 	2016/11/28 	MMA 	Oddy Test (method: 20161007_OT ), SPME GCMS	cured according to manufacturer's instructions - 7 day room temperature cure 	 	Polymer - adhesive - caulk or sealant 	 	
739 silicone sealant 	Dow Corning 	Dow Corning 	P 	2016/11/28 	MMA 	Oddy Test (method: 20161007_OT ), SPME GCMS	cured according to manufacture instructions 3 days at room temperature 	 	Polymer - adhesive - caulk or sealant 	 	
791 gray silicone building sealant 	Dow Corning 	unknown 	T 	2016/09/22 	MMA 	Oddy Test (method: 20160822_OT ), SPME GCMS	silicone sealant; Cured 22 days 	 	Polymer - adhesive - caulk or sealant 	 	
795 White silicone building sealant 	Dow Corning 	unknown 	P 	2016/09/22 	MMA 	Oddy Test (method: 20160822_OT ), SPME GCMS	silicone sealant; Cured 22 days 	 	Polymer - adhesive - caulk or sealant 	 	
795 gray silicone building sealant 	Dow Corning 	unknown 	P 	2016/07/21 	MMA 	Oddy Test (method: 20170623_OT ), SPME GCMS	silicone building sealant 	 	Polymer - adhesive - caulk or sealant 	 	
7091 black one part silicone sealant with excellent adhesion to plastics 	Dow Corning 	unknown 	P 	2017/12/21 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS	Cure start: 11/14/17 (6 day cure); product expiration date: 12/6/2017 	 	Polymer - adhesive - caulk or sealant 	 	
super 77 multipurpose spray adhesive 	3M 	unknown 	T 	2017/12/14 	MMA 	Oddy Test (method: 20171116_OT ), SPME GCMS	 	 	Polymer - adhesive - glue - liquid 	 	
OPACICOAT-300 Silicone Water Based Elastomer 	Industrial Control Development, Inc 	 	Temporary 	2018/03/06 	MMA 	Oddy Test (method: 20180206_OT), SPME GCMS 	OpaciCoat 300 with "white pure" colorant; Cured for > 7 days 	 	Coating - paint or primer 	 	
Egosilicon 460 WHITE 	EGO Dichstoffwerke GnbH & Co. Betriebs KG 	 	Pass 	2018/02/13 	MMA 	Oddy Test (method: 20171116_OT), SPME GCMS 	cured at least 24 hours; model #366; silicone sealant; 	 	Polymer - adhesive - caulk or sealant 	 	
Egosilicon 460 Black 	EGO Dichstoffwerke GnbH & Co. Betriebs KG 	 	Pass 	2018/02/13 	MMA 	Oddy Test (method: 20171116_OT), SPME GCMS 	cured at least 24 hours; model #366; silicone sealant 	 	Polymer - adhesive - caulk or sealant 	 	
Resene Lumbersider Acrylic 	Resene 	 	Suitable for permanent use 	1996/04/01 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Resene Lustacryl semi gloss water based enamel paint 	Resene 	 	Suitable for permanent use 	1997/01/01 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Resene Supergloss Interior/Exterior Enamel, White 	Resene 	 	Suitable for temporary use 	1997/02/06 	AWMM 	Oddy test 	Paints, varnishes,stains 	 	Coating - paint & primer 	 	
Alto Country Colours Cabinet Interior Acrylic 	Alto 	 	Suitable for permanent use 	1997/04/03 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Levene Goldline low sheen acrylic interior/exterior paint 	Levene 	 	Suitable for temporary use 	1997/04/03 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - paint & primer 	Suitable for use in temporary exhibition spaces only, ie up to 6 mths. Not suitable for storage spaces. 	
Resene Zylone Sheen washable wallpaint vinyl interior interior/exterior 	Resene 	 	Suitable for temporary use 	1997/04/03 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - paint & primer 	Suitable for use in temporary exhibition spaces only, ie up to 6 mths. Not suitable for storage spaces. 	
Resene Zylone sheen low sheen acrylic interior/exterior 	Resene 	 	Suitable for temporary use 	1997/04/03 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - paint & primer 	Suitable for use in temporary exhibition spaces only, i.e. up to 6 mths. Not suitable for storage spaces. 	
Resene Lumbersider Acrylic 	Resene 	 	Suitable for permanent use 	1997/05/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Resene Supergloss Interior/Exterior Enamel (oil based, white) 	Resene 	 	Not suitable for use 	1997/05/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	 	Coating - paint & primer 	 	
Resene Zylone 20 vinyl flat wallpaint interior 	Resene 	 	Suitable for permanent use 	1997/05/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	Suitable for use in temporary exhibition spaces only, i.e. up to 6 mths. Not suitable for storage spaces. 	
Resene PVA Semigloss acrylic decorator series paint 	Resene 	 	Suitable for permanent use 	1997/05/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Resene Enamacryl gloss water based enamel paint 	Resene 	 	Suitable for permanent use 	1997/05/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Resene Alkyd Satin oil based Enamel paint, Decorator series 	Resene 	 	Not suitable for use 	1997/05/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	 	Coating - paint & primer 	 	
Dulux Breatheasy low sheen interior paint 	Dulux 	 	Suitable for permanent use 	1999/02/24 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Dulux Interior Low Sheen Acrylic Wash And Wear 	Dulux 	 	Suitable for temporary use 	1999/02/24 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - paint & primer 	Slight discolouration on the silver coupon. Suitable for use with selected displays only, or for temporary use. 	
Plasti-kote premium water based enamel spray paint , Black semi-gloss 	 	 	Not suitable for use 	1999/08/15 	AWMM 	Oddy test 	Paints, varnishes,stains 	 	Coating - paint & primer 	 	
PaintPlus Colour Systems QuikPrep , White 	 	 	Suitable for permanent use 	2001/08/30 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
PaintPlus Colour Systems Scenic Flat White 	 	 	Suitable for permanent use 	2001/08/30 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
PaintPlus Colour Systems Acrynamel , White 	 	 	Suitable for temporary use 	2001/08/31 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	Suitable for temporary use – slight overall corrosion on lead coupon. 	
PaintPlus Colour Systems , Scenic Flat White 	 	 	Suitable for permanent use 	2001/09/01 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Plastikote spray primer 	 	 	Not suitable for use 	2003/01/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	 	Coating - paint & primer 	 	
Mirotec WB-8060 clear water based topcoat 	Calavera Specialist Construction and Installation 	 	Suitable for permanent use 	2014/05/07 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	Very slightly more reacted than controls, borderline acceptable. 	
Dulux Kulorthene 500ES, 9239133S, black 	Dulux powder and Industrial Coatings 	Dulux powder and Industrial Coatings 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
AO 470 Mirotone polyurethane coating, topcoat, 1K 	Industria Chimica Adriatica S.P.A. 	 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
AO 470 Mirotone polyurethane coating, topcoat, 2K 	Industria Chimica Adriatica S.P.A. 	 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
FA452B Mirotone polyurethane coating, undercoat, 1K 	Industria Chimica Adriatica S.P.A. 	 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
FA452B Mirotone polyurethane coating, undercoat, 2K 	Industria Chimica Adriatica S.P.A. 	 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
AOB510G25 Mirotone polyurethane coating, topcoat, 1K 	Industria Chimica Adriatica S.P.A. 	 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
AOB510G25 Mirotone polyurethane coating, topcoat, 2K 	Industria Chimica Adriatica S.P.A. 	 	Suitable for permanent use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Speedlac Black, PPG262 	PPG Industries New Zealand 	PPG Industries New Zealand 	Not suitable for use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
PPG849 G30 	PPG Industries New Zealand 	PPG Industries New Zealand 	Not suitable for use 	2017/05/18 	AWMM 	Oddy test 	Paints, varnishes,stains 	In vitrine or case 	Coating - paint & primer 	 	
Densi-Proof 	Protect Crete NZ Ltd 	Protect Crete NZ Ltd 	Suitable for temporary use 	2009/01/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - protective (eg. anti-UV, -abbrasion, -tarnish) 	 	
Lustre-Shield 	Protect Crete NZ Ltd 	Protect Crete NZ Ltd 	Suitable for permanent use 	2009/01/12 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - protective (eg. anti-UV, -abbrasion, -tarnish) 	 	
Pinnacle (wet), cloudy, colourless 	JohnsonDiversey 	 	Suitable for temporary use 	2013/10/16 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - protective (eg. anti-UV, -abbrasion, -tarnish) 	 	
Pinnacle (redone, dried) 	JohnsonDiversey 	 	Suitable for temporary use 	2013/10/16 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Coating - protective (eg. anti-UV, -abbrasion, -tarnish) 	 	
Sika remover 208 	Hydestor 	Hydestor 	Suitable for permanent use 	2013/03/13 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Other - stripper 	 	
Sika remover 208 	Hydestor 	Hydestor 	Suitable for permanent use 	2013/03/13 	AWMM 	Oddy test 	Paints, varnishes,stains 	Outside vitrine or case 	Other - stripper 	 	
Sikaflex AT façade,wet sealant 	Hydestor 	Hydestor 	Suitable for permanent use 	2013/03/13 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Coating - paint & primer 	 	
Sikaflex AT façade, wet sealant 	Hydestor 	Hydestor 	Suitable for permanent use 	2013/03/13 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Coating - paint & primer 	 	
Sikaflex AT façade, dry sealant 	Hydestor 	Hydestor 	Suitable for permanent use 	2013/03/13 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Coating - paint & primer 	 	
Sikaflex AT façade, dry sealant 	Hydestor 	Hydestor 	Suitable for permanent use 	2013/03/13 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Coating - paint & primer 	 	
Mirotec WB-8022 clear water based sealer 	Calavera Specialist Construction and Installation 	 	Suitable for permanent use 	2014/05/07 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	In vitrine or case 	Coating - paint & primer 	Very slightly more reacted than controls, borderline acceptable. 	
3M Barrier CP25WB+ Sealant, red 	3M 	 	Suitable for permanent use 	2014/03/06 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Other - fire barrier 	 	
Silastic 1080 Silicone RTV adhesive sealant 	Dow Corning 	 	Suitable for permanent use 	1998/07/20 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Polymer - adhesive - caulk or sealant 	 	
3145 RTV MIL-A-46146 Adhesive Sealant 	Dow Corning 	 	Suitable for permanent use 	1998/07/20 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Polymer - adhesive - caulk or sealant 	 	
Selleys All Clear Universal CoPolymer Sealant 	Sellys 	 	Not suitable for use 	1999/02/24 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	 	Polymer - adhesive - caulk or sealant 	 	
Selleys Roof and Gutter Silicone Sealer , Clear 	Sellys 	 	Suitable for permanent use 	1999/02/24 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Polymer - adhesive - caulk or sealant 	 	
Dow Corning 580 glass, metal and masony silicone sealant, Translucent 580 	Dow Corning 	 	Suitable for temporary use 	2007/11/29 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Polymer - adhesive - caulk or sealant 	 	
795 Silicone Building Sealant, neutral one part silicone, black 	Dow Corning 	 	Not suitable for use 	2008/02/28 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	 	Polymer - adhesive - caulk or sealant 	Suitable for permanent use for large showcases as joint sealant /support for glass and panel materials. Not suitable in small showcases under 1m3 displaying metal objects or when in direct contact with artifacts)	
580 Glass, Metal & Masonry silicone sealant, Dow Corning, 580, translucent 	Glasscorp Auckland 	Glasscorp Auckland 	Suitable for temporary use 	2008/03/04 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	In vitrine or case 	Polymer - adhesive - caulk or sealant 	 	
380 Glazing and Partition Sealant, Dow Corning, transparent, neutral cure 	Glasscorp Auckland 	Glasscorp Auckland 	Not suitable for use 	2008/03/04 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	 	Polymer - adhesive - caulk or sealant 	Suitable for permanent use as joint sealant for glass and panel materials. Not suitable for mounts or when in direct with artefacts in particular lead and copper objects. 	
Selleys Brick and Concrete Silicone Sealer , Opaque 	Sellys 	 	Suitable for permanent use 	1999/05/24 	AWMM 	Oddy test 	Adhesives, consolidants, sealants 	Outside vitrine or case 	Coating - protective (eg. anti-UV, -abbrasion, -tarnish) 	 	
Regal Classic Interior 100% Acrylic Paint Semi-Gloss Finish Medium Base N3332B 	Benjamin Moore 	 	Temporary 	2016/06/08 	CAM 	Oddy 	100% Acrylic Paint Semi-Gloss Finish Medium Base N3332B 	for use as interior paint; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - Darkened, Pb - light grey in middle 	
Regal Select Eggshell Finish Base 4 S494X 	Benjamin Moore 	 	Pass 	2016/06/08 	CAM 	Oddy 	Eggshell Finish Base 4 S494X 	for use as interior paint; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - Slight darkening, Pb - slight grey in middle 	
Dow Guard 	Dow Chemical 	Dow Chemical 	Short-term 	2006/01/19 	CAM 	Oddy 	 	for use in exhibit cases; test run at 60 ˚C for 8 weeks 	paint/coating 	Description: Ag - Slight to moderate darkening, Cu - Severe multicolotred tarnishing, Pb - Dark grey 	
Crystal Clear 	Krylon Products Group 	Krylon Products Group 	Fail 	2015/07/28 	CAM 	Oddy 	Acrylic Coating 1303 	for use as coating; test run at 65 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - dark brown specks and dark purple appearance, Pb - hazy bluish corrosion 	
Crystal Clear 	Krylon Products Group 	Krylon Products Group 	Retest 	2016/05/25 	CAM 	Oddy 	Acrylic Coating 1304 	for use as coating; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - Tarnish, Pb - Grey spots 	
Crystal Clear 	Krylon Products Group 	Krylon Products Group 	Short-term 	2016/07/01 	CAM 	Oddy 	Acrylic Coating 1305 	for use as coating; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - Uneven darkening, Pb - Tarnish 	
PureBond + Sancure+ Pure Performance 	 	 	Pass 	2007/01/31 	CAM 	Oddy 	 	for use in exhibit cases; test run at 60 ˚C for 4 weeks 	substrate with paint/coating 	Description: Ag - good, Cu - very slight oragne tone, Pb - moderate white haze 	
Sancure 878 	Noveon 	 	PASS 	2006/09/29 	CAM 	Oddy 	Aliphatic Waterborne Urethane Polymer 	for use in exhibit cases; test run at 60 ˚C for 3 weeks 	coating 	Description: Ag - corrosion associated with H2O, Cu - shiny- OK, Pb - slightly darker 	
Sancure 878 	Noveon 	 	PASS 	2006/09/29 	CAM 	Oddy 	Aliphatic Waterborne Urethane Polymer 	for use in exhibit cases; test run at 60 ˚C for 4 weeks 	coating 	Description: Ag - shiny-ok, Cu - corrosion associated w H2O, Pb - heavier corrosion near H2O 	
Sancure 878 	Noveon 	 	Pass 	2007/01/31 	CAM 	Oddy 	Aliphatic Waterborne Urethane Polymer 	for use as coating; test run at 60 ˚C for 4 weeks 	coating 	Description: Ag - good, Cu - good, Pb - slight darkening 	
Porter Flat wall Paint 	Porter 	Porter 	Pass 	2007/01/31 	CAM 	Oddy 	 	for use as interior paint; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - good, Cu - slight tarnishing, Pb - slight darkening 	
Pure Performance Acrylic latex CAM 17 	Pittsburgh Paints 	Porter 	Retest 	2006/09/29 	CAM 	Oddy 	Acrylic latex CAM 17 	for use in exhibit cases; test run at 60 ˚C for 3 weeks 	paint/coating 	Description: Ag - slightly dull at edges, Cu - slight darkening, Pb - dark overall 	
Pure Performance Acrylic latex CAM 17 	PPG Paints 	Porter 	Retest 	2006/09/29 	CAM 	Oddy 	Acrylic latex CAM 17 	for use in exhibit cases; test run at 60 ˚C for 3 weeks 	paint/coating 	Description: Ag - shiny-ok, Cu - slight darkening, Pb - dark overall 	
Pure Performance Acrylic latex CAM 17 	Pittsburgh Paints 	Porter 	Pass 	2007/01/31 	CAM 	Oddy 	Acrylic latex CAM 18 	for use in exhibit cases; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - good, Cu - very slight, Pb - very slight 	
Pure Performance Acrylic Latex Eggshell 9-340 Ultra Deep Base 	PPG Paints 	Porter 	Pass 	2016/06/08 	CAM 	Oddy 	Acrylic Latex Eggshell 9-340 Ultra Deep Base 	for use in walls and cases; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - no change, Pb - slight grey in middle 	
Super Premim Silken Touch Interior Eggshell Latex Ultra Deep Base pp999-40 	PPG Paints 	Porter 	Temporary 	2016/06/08 	CAM 	Oddy 	Interior Eggshell Latex Ultra Deep Base pp999-40 	for use in walls and cases; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - no change, Pb - corrosion 	
Emerald Interior Acrylic Latex Ultra Deep Base Matte 	Sherwin Williams 	Sherwin Williams 	Pass 	2016/06/08 	CAM 	Oddy 	Interior Acrylic Latex Ultra Deep Base Matte 	for use in walls and cases; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - no change, Pb - slight grey patches in middle 	
to LIMN 4711 white 	to LIMN 	To LIMN 	Fail 	2009/05/18 	CAM 	Oddy 	4710 white 	for use in walls and cases; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - darken overall, slight purple irridescence, Pb - very light gray overall with a band of white 	
to LIMN 4711 white 	to LIMN 	To LIMN 	Short-term 	2009/05/18 	CAM 	Oddy 	4711 white 	for use in walls and cases; test run at 60 ˚C for 4 weeks 	paint/coating 	Description: Ag - no change, Cu - darken overall, Pb - hazy gray overall. Band of white corossion. 	
BEN Latex Interior, W625-4X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 4 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
BEN Latex Interior, W625-3X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 3 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
BEN Latex Interior, W625-2X 	Benjamin Moore 	Jill's Paint 	Temporary pass no Cu-alloys	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 2 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
BEN Latex Interior, W625-1X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 1 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
Regal Select Latext Interior, W547-4X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 4 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
Regal Select Latext Interior, W547-3X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 3 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
Regal Select Latext Interior, W547-2X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 2 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
Regal Select Latext Interior, W547-1X 	Benjamin Moore 	Jill's Paint 	F 	2014 Oct/Nov	Autry 	Oddy Test 	Flat Base 1 	Pigment-less base painted onto plastic sheeting and peeled up, Drying time: 4 weeks 	COATING, PAINT 	none 	
SAFE COAT SEMI GLOSS, 80290 	AFM SAFECOAT 	AFM SAFECOAT 	T 	2009/06/29 	BM 	Oddy Test 	ACRYLIC EMULSION, WHITE 	Drying time: 4 WEEKS, test #6520 	COATING, PAINT 	none 	
SAFE SEAL MDF SEALER, 3104 	AFM SAFECOAT 	AFM SAFECOAT 	T 	2009/06/29 	BM 	Oddy Test 	ACRYLIC PIGMENTED POLYMER EMULSION, CLEAR 	Drying time: 4 WEEKS, test #6540 	COATING, PRIMER 	none 	
DULUX LIFEMASTER EGGSHELL, 30BB 10/112 SIGNAUTRE BLUE 	AKAO NOBEL CANADA (M) 	DULUX PAINT STORE (S) TORONTO 	P 	2013/03/02 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #7820 	COATING, PAINT 	none 	
DULUX LIFEMASTER EGGSHELL, 45YY 83/062 STONE WHITE 	AKAO NOBEL CANADA (M) 	DULUX PAINT STORE (S) TORONTO 	P 	2013/03/02 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7821 	COATING, PAINT 	none 	
INTERPON POWDER COAT PAINT, 3002 	AKZO NOBEL 	AKZO NOBEL 	P 	2010/04/15 	BM 	Oddy Test 	POWDER COAT PAINT, RED 	Drying time: BAKED, test #6808 	COATING, POWDER 	none 	
INTERPON POWDER COAT PAINT, 9005 	AKZO NOBEL 	AKZO NOBEL 	P 	2010/04/15 	BM 	Oddy Test 	POWDER COAT PAINT, BLUE 	Drying time: BAKED, test #6809 	COATING, POWDER 	none 	
ECO SPEC WB INTERIOR LATEX EGGSHELL FINISH BASE 1, OC-17 WHITE DOVE 	BENJAMIN MOORE (M) 	PAINT COLOURS UNLIMITED (S) TORONTO 	P 	2013/03/02 	BM 	Oddy Test 	ACRYLIC EMULSION, WHITE 	Drying time: 4 WEEKS, test #7823 	COATING, PAINT 	none 	
NATURA INTERIOR WATERBORNE EGGSHELL, AF-645 CHAMBOURD 	BENJAMIN MOORE (M) 	PAINT COLOURS UNLIMITED (S) TORONTO 	P 	2013/03/02 	BM 	Oddy Test 	ACRYLIC EMULSION, PURPLE, DARK 	Drying time: 4 WEEKS, test #7822 	COATING, PAINT 	none 	
QUALICOAT PAINT, RAL 7024 MATT 	BSO METALLVEREDERLUNG 	BSO METALLVEREDERLUNG 	P 	2013/06/26 	BM 	Oddy Test 	POWDER COATING PAINT, GREY, DARK 	Drying time: N/A, test #7890 	COATING, POWDER 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 21-31T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, PURPLE 	Drying time: 4 WEEKS, test #7517 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 23-30T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, PURPLE 	Drying time: 4 WEEKS, test #7523 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 23-31T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, GREY 	Drying time: 4 WEEKS, test #7522 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 24-30T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, BLUE 	Drying time: 4 WEEKS, test #7519 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 38-32T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, GREEN 	Drying time: 4 WEEKS, test #7524 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 42-31T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, GREEN 	Drying time: 4 WEEKS, test #7518 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 42-32T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, GREEN 	Drying time: 4 WEEKS, test #7516 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, 48-32T 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, BROWN 	Drying time: 4 WEEKS, test #7520 	COATING, PAINT 	none 	
SANDERSON SPECTRUM PAINT, 42-30 T, OLD LEAF 	CROWN PAINTS (M) 	C BREWER & SONS (S) 	P 	2011/03/16 	BM 	Oddy Test 	ACRYLIC EMULSION, GREEN 	Drying time: 4 WEEKS, test #7228 	COATING, PAINT 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, BLUE, DARK 	CROWN PAINTS LTD (M) 	LEYLAND SDM (S) 	T 	2013/07/08 	BM 	Oddy Test 	SHOWCASE, VINYL EMULSION 	Drying time: L9072W, test #7896 	CROWN PAINTS LTD (M) 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, GREY, DARK 	CROWN PAINTS LTD (M) 	LEYLAND SDM (S) 	T 	2013/07/08 	BM 	Oddy Test 	SHOWCASE, VINYL EMULSION 	Drying time: B4070C, test #7895 	CROWN PAINTS LTD (M) 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, PURPLE, DARK 	CROWN PAINTS LTD (M) 	LEYLAND SDM (S) 	F 	2013/07/08 	BM 	Oddy Test 	SHOWCASE, VINYL EMULSION 	Drying time: W1081M, test #7893 	CROWN PAINTS LTD (M) 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, PURPLE, DARK 	CROWN PAINTS LTD (M) 	LEYLAND SDM (S) 	T 	2013/07/08 	BM 	Oddy Test 	SHOWCASE, VINYL EMULSION 	Drying time: U7062E, test #7894 	CROWN PAINTS LTD (M) 	none 	
CROWN TRADE CT COLOUR COLLECTION MATT, PURPLE, DARK 	CROWN PAINTS LTD (M) 	LEYLAND SDM (S) 	F 	2013/07/08 	BM 	Oddy Test 	SHOWCASE, VINYL EMULSION 	Drying time: W5061H, test #7897 	CROWN PAINTS LTD (M) 	none 	
DACRYLATE GLOSS VARNISH, 103-1 	DACRYLATE PAINTS, LTD. 	DACRYLATE PAINTS, LTD. 	P 	2013/04/19 	BM 	Oddy Test 	ACRYLIC EMULSION, CLEAR 	Drying time: 4 WEEKS, test #7767 	COATING, VARNISH 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 0036 MARS BLACK 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLACK 	Drying time: 4 WEEKS, test #6370 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 009 TITANIUM WHITE 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, WHITE 	Drying time: 4 WEEKS, test #6369 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 111 COERULEUM 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLUE 	Drying time: 4 WEEKS, test #6372 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 123 ULTRAMARINE 	DALER-ROWNEY 	DALER-ROWNEY 	F 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLUE 	Drying time: 4 WEEKS, test #6371 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 221 BURNT SIENNA 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN, DARK 	Drying time: 4 WEEKS, test #6366 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 223 BURNT UMBER 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN, DARK 	Drying time: 4 WEEKS, test #6365 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 247 RAW UMBER 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN 	Drying time: 4 WEEKS, test #6363 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 501 CADMIUM RED 	DALER-ROWNEY 	DALER-ROWNEY 	T 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, RED 	Drying time: 4 WEEKS, test #6367 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 525 CRIMSON ALIZARIN 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, RED 	Drying time: 4 WEEKS, test #6368 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 612 CADMIUM YELLOW 	DALER-ROWNEY 	DALER-ROWNEY 	T 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW 	Drying time: 4 WEEKS, test #6362 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 651 LEMON YELLOW 	DALER-ROWNEY 	DALER-ROWNEY 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW, LIGHT 	Drying time: 4 WEEKS, test #6361 	COATING, PAINT 	none 	
DALER-ROWNEY CRYLA ARTISTS' HEAVY BODY ACRYLIC COLOUR, 663 YELLOW OCHRE 	DALER-ROWNEY 	DALER-ROWNEY 	T 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW, DARK 	Drying time: 4 WEEKS, test #6364 	COATING, PAINT 	none 	
skywhite paint 	Delta Design 	Unknown 	Pass 	2000/09/19 	GCI 	Oddy 	white paint 	tested for gallery walls 	paint, water based 	n/a 	
TRANSPARENT NONCORROSIVE SILICONE ADHESIVE SEALANT, AS 7096N 	DOW CORNING 	DOW CORNING 	P 	2009/09/16 	BM 	Oddy Test 	SILICONE ADHESIVE, CLEAR 	Drying time: 24 HRS, test #6605 	SEALANT 	none 	
DOW CORNING ADHSIVE SELANT, 799 	DOW CORNING (M) 	CONSERVATION BY DESIGN (S) 	P 	2013/01/18 	BM 	Oddy Test 	NEUTRAL 1 PART SILICONE SEALANT, WHITE 	Drying time: 48HRS, test #7680 	SEALANT 	none 	
DOW CORNING , 993 2K 	DOW CORNING (M) 	DOW CORNING 	T 	2013/03/22 	BM 	Oddy Test 	SILICON, BLACK 	Drying time: 48 HOURS, test #7738 	SEALANT 	none 	
ASCODUR SF HV POLYURETHANE SOFT FEEL COAT, RAL7024 	DR. A, SCHOCH AG/ LEO LACHENNER MALERGESSCHAFT 	DR. A, SCHOCH AG/ LEO LACHENNER MALERGESSCHAFT 	T 	2010/07/19 	BM 	Oddy Test 	POLYURETHANE, BLACK 	Drying time: 4 WEEKS, test #6903 	COATING, PAINT 	none 	
CLAYPAINT, 3-1211 	EARTH BORN 	EARTH BORN 	P 	2009/06/29 	BM 	Oddy Test 	CLAY PAINT, WHITE 	Drying time: 4 WEEKS, test #6523 	COATING, PAINT 	none 	
PRO AQUA EGGSHELL, 2-3792 	EARTH BORN 	EARTH BORN 	P 	2009/06/29 	BM 	Oddy Test 	WATER BASED EMULSION, WHITE 	Drying time: 4 WEEKS, test #6530 	COATING, PAINT 	none 	
ATMOSPHERE PURIFYING WALL PAINT, 	ECOS 	ECOS 	P 	2009/06/29 	BM 	Oddy Test 	EMULSION, WHITE 	Drying time: 4 WEEKS, test #6522 	COATING, PAINT 	none 	
MDF PASSIVATING PRIMER, 	ECOS 	ECOS 	P 	2009/06/29 	BM 	Oddy Test 	EMULSION, WHITE 	Drying time: 4 WEEKS, test #6533 	COATING, PRIMER 	none 	
FARROW & BALL ESTATE EMULSION, 1 LIME WHITE 	FARROW & BALL(M) 	C BREWER & SONS (S) 	F 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, CREAM 	Drying time: 4 WEEKS, test #7489 	COATING, PAINT 	none 	
FARROW & BALL ESTATE EMULSION, 2003 POINTING 	FARROW & BALL(M) 	C BREWER & SONS (S) 	F 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, WHITE 	Drying time: 4 WEEKS, test #7488 	COATING, PAINT 	none 	
FARROW & BALL ESTATE EMULSION, 2005 ALL WHITE 	FARROW & BALL(M) 	C BREWER & SONS (S) 	F 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, WHITE 	Drying time: 4 WEEKS, test #7491 	COATING, PAINT 	none 	
FARROW & BALL ESTATE EMULSION, 2009 CLUNCH 	FARROW & BALL(M) 	C BREWER & SONS (S) 	F 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, CREAM 	Drying time: 4 WEEKS, test #7490 	COATING, PAINT 	none 	
FARROW & BALL ESTATE EMULSION, 2010 JAMES WHITE 	FARROW & BALL(M) 	C BREWER & SONS (S) 	T 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, CREAM 	Drying time: 4 WEEKS, test #7492 	COATING, PAINT 	none 	
FARROW & BALL ESTATE EMULSION, 43 EATING ROOM RED 	FARROW & BALL(M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	VINYL EMULSION, RED 	Drying time: 4 WEEKS, test #7521 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/ PW6 TITANIUM WHITE 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, WHITE 	Drying time: 4 WEEKS, test #6375 	 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/1020-2/PBR7 BURNT SIENNA 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN, DARK 	Drying time: 4 WEEKS, test #6374 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/1030-2/PBR7 BURNT UMBER 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN 	Drying time: 4 WEEKS, test #6381 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/1340-2/PY43 RAW SIENNA 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN, LIGHT 	Drying time: 4 WEEKS, test #6373 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/1350-2/PBR7 RAW UMBER 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BROWN 	Drying time: 4 WEEKS, test #6382 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/1407-2/PY43 YELLOW OCHRE 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW, DARK 	Drying time: 4 WEEKS, test #6380 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/PBK11 MARS BLACK 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLACK 	Drying time: 4 WEEKS, test #6376 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 1/PR112 NAPTHOL RED LIGHT 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, RED 	Drying time: 4 WEEKS, test #6379 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 2/PB29 ULTRAMARINE 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLUE 	Drying time: 4 WEEKS, test #6383 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 3/PY73 HANSA YELLOW MEDIUM 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW 	Drying time: 4 WEEKS, test #6377 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 4/1554-2 PY83/PY53/PY3 CADMIUM YELLOW MEDIUM 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW 	Drying time: 4 WEEKS, test #6378 	COATING, PAINT 	none 	
GOLDEN HEAVY BODY ACRYLICS, SERIES 4/P43/PG7 PERMANENT GREEN LIGHT 	GOLDEN ARTIST COLOURS INC. (M) 	LONDON GRAPHICS CENTRE (S) 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, GREEN, LIGHT 	Drying time: 4 WEEKS, test #6384 	COATING, PAINT 	none 	
HALFORDS ENAMEL MATT SPRAY PAINT, ARTICELCODE: 155666 	HALFORDS 	HALFORDS 	T 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, WHITE 	Drying time: 4 WEEKS, test #6983 	COATING, PAINT 	none 	
HALFORDS ENAMEL MATT SPRAY PAINT, ARTICELCODE: 155724 	HALFORDS 	HALFORDS 	T 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, BLACK 	Drying time: 4 WEEKS, test #6985 	COATING, PAINT 	none 	
HALFORDS ENAMEL MATT SPRAY PAINT, ARTICELCODE: 451583 	HALFORDS 	HALFORDS 	T 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, BLACK 	Drying time: 4 WEEKS, test #6984 	COATING, PAINT 	none 	
HALFORDS ENAMEL SPRAY PAINT, ARTICELCODE: 156581 	HALFORDS 	HALFORDS 	P 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, GREY 	Drying time: 4 WEEKS, test #6987 	COATING, PAINT 	none 	
HALFORDS PRIMER SPRAY PAINT, ARTICELCODE: 451542 	HALFORDS 	HALFORDS 	T 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, GREY 	Drying time: 4 WEEKS, test #6986 	COATING, PAINT 	none 	
HALFORDS PRIMER SPRAY PAINT, ARTICELCODE: 473124 	HALFORDS 	HALFORDS 	P 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, WHITE 	Drying time: 4 WEEKS, test #6982 	COATING, PAINT 	none 	
HAMMERITE DIRECT TO RUST METAL PAINT, 	HAMMERITE 	HAMMERITE 	F 	2009/06/29 	BM 	Oddy Test 	SOLVENT BASED, WHITE 	Drying time: 4 WEEKS, test #6537 	COATING, PAINT 	none 	
TEROSTAT, 9220 	HENKEL TEROSON 	HENKEL TEROSON 	P 	2012/10/26 	BM 	Oddy Test 	MS POLYMER, BLACK 	Drying time: 48 HOURS, test #7644 	SEALANT 	none 	
MORELLI SPRAY PAINT, RAL 7030 stone grey 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, GREY 	Drying time: 4 WEEKS, test #6837 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL 7037 dusty grey 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, GREY 	Drying time: 4 WEEKS, test #6838 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL 9001 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, CREAM 	Drying time: 4 WEEKS, test #6834 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL 9003 signal white 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, WHITE 	Drying time: 4 WEEKS, test #6836 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL 9004 matt black 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, BLACK 	Drying time: 4 WEEKS, test #6840 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL 9004 signal black gloss 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, BLACK 	Drying time: 4 WEEKS, test #6841 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL 9010 pure white 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, WHITE 	Drying time: 4 WEEKS, test #6835 	COATING, PAINT 	none 	
MORELLI SPRAY PAINT, RAL7022 umber grey 	HMG PAINTS 	HMG PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	, GREY 	Drying time: 4 WEEKS, test #6839 	COATING, PAINT 	none 	
NAUTECO MDF SEALER, F2014 	HMG PAINTS 	HMG PAINTS 	T 	2009/06/29 	BM 	Oddy Test 	, WHITE 	Drying time: 4 WEEKS, test #6524 	COATING, PRIMER 	none 	
HUMBROL ACRYLIC SPRAY PAINT, WHITE MATT 34 	HORNBY HOBBIES KENT 	HORNBY HOBBIES KENT 	T 	2012/06/06 	BM 	Oddy Test 	ACRYLIC, WHITE 	Drying time: BAKED 60C/24 HRS, test #7545 	COATING, PAINT 	none 	
DULUX ENVIRO 2 PREMIUM LOW SHEEN ACRYLIC, PW2.B5 	ICI PAINTS 	ICI PAINTS 	P 	2009/02/13 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #6349 	COATING, PAINT 	none 	
DULUX ENVIRO 2 PREMIUM LOW SHEEN ACRYLIC, PW2.D4 	ICI PAINTS 	ICI PAINTS 	P 	2009/02/13 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #6348 	COATING, PAINT 	none 	
DULUX PROFESSIONAL 1-STEP PRIMER, SEALER AND UNDERCOAT, 	ICI PAINTS 	ICI PAINTS 	P 	2009/02/13 	BM 	Oddy Test 	ACRYLIC, CREAM 	Drying time: 4 WEEKS, test #6351 	COATING, PRIMER 	none 	
DULUX TRADE DIAMOND EGGSHELL EMULSION, 5502B BATTLESHIP 	ICI PAINTS 	ICI PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #6831 	COATING, PAINT 	none 	
DULUX TRADE DIAMOND EGGSHELL EMULSION, OOE53 	ICI PAINTS 	ICI PAINTS 	F 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLACK 	Drying time: 4 WEEKS, test #6832 	COATING, PAINT 	none 	
DULUX TRADE DIAMOND EGGSHELL EMULSION, PURE BRILLIANT WHITE 	ICI PAINTS 	ICI PAINTS 	P 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #6829 	COATING, PAINT 	none 	
DULUX TRADE DIAMOND QUICK DRYING EGGSHELL, LIGHT W26 	ICI PAINTS 	ICI PAINTS 	T 	2009/02/12 	BM 	Oddy Test 	ACRYLIC COPOLYMER, WATER-BASED, BEIGE 	Drying time: 4 WEEKS, test #6192 	COATING, PAINT 	none 	
DULUX TRADE FLAT MATT EMULSION, 00YY09087 	ICI PAINTS 	ICI PAINTS 	P 	2009/11/23 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #6654 	COATING, PAINT 	none 	
DULUX TRADE FLAT MATT EMULSION, 10YY 08093 	ICI PAINTS 	ICI PAINTS 	P 	2009/11/23 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #6658 	COATING, PAINT 	none 	
DULUX TRADE FLAT MATT EMULSION, 48YR 06091 	ICI PAINTS 	ICI PAINTS 	P 	2009/11/23 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #6657 	COATING, PAINT 	none 	
DULUX TRADE FLAT MATT EMULSION, 50YR 09162 	ICI PAINTS 	ICI PAINTS 	P 	2009/11/23 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #6659 	COATING, PAINT 	none 	
DULUX TRADE FLAT MATT EMULSION, 70YR 07093 	ICI PAINTS 	ICI PAINTS 	P 	2009/11/23 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #6656 	COATING, PAINT 	none 	
DULUX TRADE FLAT MATT EMULSION, 80YR 09163 	ICI PAINTS 	ICI PAINTS 	T 	2009/11/23 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #6655 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 00NN16000, ICE STORM 2 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #7200 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 10BG21141 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7497 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 10YY83071 	ICI PAINTS 	ICI PAINTS 	P 	2011/11/09 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7329 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30BG23124 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7496 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30GG29196 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7493 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30GG33275 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7494 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30YR07157, BITTER CHOCOLATE 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #7201 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 40YY67087 BLEACHED LINEN 	ICI PAINTS 	ICI PAINTS 	P 	2012/03/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #7404 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 40YY75084 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #7499 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 4YY74056 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #7498 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 502YR50R 	ICI PAINTS 	ICI PAINTS 	P 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #6830 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 50GG43213 	ICI PAINTS 	ICI PAINTS 	F 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7495 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 50RR26361 	ICI PAINTS 	ICI PAINTS 	F 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PINK, DARK 	Drying time: 4 WEEKS, test #7025 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 5502B BATTLESHIP 	ICI PAINTS 	ICI PAINTS 	P 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #6827 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, OOE53 	ICI PAINTS 	ICI PAINTS 	T 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLACK 	Drying time: 4 WEEKS, test #6828 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, PURE BRILLIANT WHITE 	ICI PAINTS 	ICI PAINTS 	P 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #6826 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, RO2Y50R 	ICI PAINTS 	ICI PAINTS 	P 	2010/06/07 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #6825 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, S1502Y50R 	ICI PAINTS 	ICI PAINTS 	P 	2012/10/02 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7630 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, S15O2R 	ICI PAINTS 	ICI PAINTS 	P 	2012/10/02 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7628 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, S200250R 	ICI PAINTS 	ICI PAINTS 	P 	2012/10/02 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7629 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 00NN13000, NIGHT JEWELS 	ICI PAINTS 	ICI PAINTS 	T 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #6958 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 09YR11475 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/09 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: BAKED 12H/60°C + AIR DRIED 12 H, test #7196 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 10BB09155 	ICI PAINTS 	ICI PAINTS 	T 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #6970 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 10RB08125, AMETHYST FALLS 1 RV 3 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7223 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 10YR07125, COCOA BLUSH 2 RN2 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7212 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 10YR09250 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7218 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 11YR07229, VOLCANIC SPLASH 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED, DARK 	Drying time: 4 WEEKS, test #6946 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 12YR07279 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7239 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 13YR07157, HOT PAPRIKA 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED, DARK 	Drying time: 4 WEEKS, test #6944 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 14YR10434, VOLCANIC SPLASH 2 RO 2 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7219 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30RR12281 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED, DARK 	Drying time: 4 WEEKS, test #7029 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30RR13328 	ICI PAINTS 	ICI PAINTS 	T 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PINK, DARK 	Drying time: 4 WEEKS, test #7051 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30YR11219 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7220 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30YY08082 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7225 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 31YR10591 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7237 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 33BG14023, RAL 7012 	ICI PAINTS 	ICI PAINTS 	F 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #6956 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 40YY08107 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7202 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 40YY08107 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7231 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 47BB09031, RAL 7024 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #6954 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 5030R90B, HIGH TIDE 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #6964 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50BB08171, SAPPHIRE SPRINGS 	ICI PAINTS 	ICI PAINTS 	T 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #6966 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50BB10112 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7221 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50BG14036 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7227 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50RB12174 	ICI PAINTS 	ICI PAINTS 	T 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE, DARK 	Drying time: 4 WEEKS, test #7027 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50RR15400 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PINK, DARK 	Drying time: 4 WEEKS, test #7037 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50YR09244, MEXICAN MOSAIC 1 RG01 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7217 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50YY47053 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7211 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70BB07103 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #7199 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70RB10157 	ICI PAINTS 	ICI PAINTS 	P 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7095 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70RB11196, HIMALAYAN MUSK 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE, DARK 	Drying time: 4 WEEKS, test #7049 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70RB18117, MELLOW HEATHER 1 	ICI PAINTS 	ICI PAINTS 	P 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7093 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70RR10140 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7216 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70YY06088 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7224 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 72RR07173 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7214 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 78RR06137 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7213 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 82BG08029, RAL 7016 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #6952 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 83BB07202, PLUSH VELVET 1 RV2 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7222 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 90BB09186 	ICI PAINTS 	ICI PAINTS 	F 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #6948 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 90BG10067 	ICI PAINTS 	ICI PAINTS 	T 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #6968 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 90YY07093, TARRAGON GLORY 1 RG 1 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #7226 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 93GY10014, RAL 7043 	ICI PAINTS 	ICI PAINTS 	F 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, DARK 	Drying time: 4 WEEKS, test #6960 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 98RR06206 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7215 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 98RR10318 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7238 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, Blush rambler 1, 50RR13343 	ICI PAINTS 	ICI PAINTS 	P 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PINK 	Drying time: 4 WEEKS, test #7085 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, FIRE CRACKER 2 	ICI PAINTS 	ICI PAINTS 	P 	2009/04/13 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #6407 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, HOT PAPRIKA 4 	ICI PAINTS 	ICI PAINTS 	P 	2009/04/13 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #6403 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, RUBY FOUNTAIN 2 	ICI PAINTS 	ICI PAINTS 	P 	2009/04/13 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #6405 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, VOLCANIC SPLASH 3 	ICI PAINTS 	ICI PAINTS 	P 	2009/04/13 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #6404 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 00YY47036 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7039 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 0500N, JABOT 	ICI PAINTS 	ICI PAINTS 	F 	2011/07/25 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7283 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 1005R50B, FASHION FINISH 	ICI PAINTS 	ICI PAINTS 	F 	2011/07/25 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7281 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30BB10019 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7209 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30BB72003 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7236 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30BG72017, CLOUDED PEARL 1 FN 8 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7233 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30YY53125 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BEIGE 	Drying time: 4 WEEKS, test #7041 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30YY56060 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7210 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30YY68024 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7235 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30YY78018 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7232 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 40YY41054 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7207 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 40YY51084 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7043 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 50BG72006 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7234 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 50RR43228 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PINK 	Drying time: 4 WEEKS, test #7033 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 50YY57082 	ICI PAINTS 	ICI PAINTS 	T 	2011/03/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7208 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 70YY46053, GREY TOPE 	ICI PAINTS 	ICI PAINTS 	P 	2011/03/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7198 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 80YR50085 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7031 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, SO300N 	ICI PAINTS 	ICI PAINTS 	F 	2011/07/25 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7280 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 10BB18106 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #6972 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 30YY51098, CHALKY DOWNS 	ICI PAINTS 	ICI PAINTS 	P 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7089 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 34GY23002, RAL 7037 	ICI PAINTS 	ICI PAINTS 	P 	2010/09/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #6950 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 4030R90B, PERSONALITY 	ICI PAINTS 	ICI PAINTS 	T 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, LIGHT 	Drying time: 4 WEEKS, test #6962 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 40YY65061 	ICI PAINTS 	ICI PAINTS 	P 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #7087 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 5005R50B 	ICI PAINTS 	ICI PAINTS 	F 	2011/07/25 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7282 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 50RB18149 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7047 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 50RB27126 	ICI PAINTS 	ICI PAINTS 	P 	2011/01/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7035 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 50RR23282, BLUSH RAMBLER 2 	ICI PAINTS 	ICI PAINTS 	T 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PINK 	Drying time: 4 WEEKS, test #7083 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 70RB31090, MELLOW HEATHER 2 	ICI PAINTS 	ICI PAINTS 	P 	2010/12/22 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7091 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 90BG38185, LUNA LANDSCAPE 	ICI PAINTS 	ICI PAINTS 	T 	2010/09/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, LIGHT 	Drying time: 4 WEEKS, test #6974 	COATING, PAINT 	none 	
DULUX WEATHER SHIELD EXTERIOR GLOSS, PURE BRILLIANT WHITE 	ICI PAINTS 	ICI PAINTS 	F 	2009/06/29 	BM 	Oddy Test 	POLYMER WITH PROPYLENE GLYCOL, WHITE 	Drying time: 4 WEEKS, test #6534 	COATING, PAINT 	none 	
DULUX WEATHER SHIELD EXTERIOR SATIN, PURE BRILLIANT WHITE 	ICI PAINTS 	ICI PAINTS 	T 	2009/06/29 	BM 	Oddy Test 	POLYMER WITH PROPYLENE GLYCOL, WHITE 	Drying time: 4 WEEKS, test #6535 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 00NN13000 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7505 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 00NN25000 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7500 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 00NN31000 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7510 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 00NN53000 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7508 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 00NN72000 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7513 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 04YR11537 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7698 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 07YR10489 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7699 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 10BB08200 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7507 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 10BB11123 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/12/28 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7673 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 11RR07229 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #7511 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30BB08188 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7506 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30BG64072 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7694 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30RR08044 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE 	Drying time: 4 WEEKS, test #7512 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30RR17034 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7515 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30YR22059 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7501 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30YY10038 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN 	Drying time: 4 WEEKS, test #7502 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30YY14070 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7504 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30YY20029 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7509 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 30YY33047 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7503 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 50BG10175 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/12/28 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7674 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 50GB08021 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/12/28 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #7670 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 70BG 56061 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7696 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 70BG 68056 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7695 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 70BG07086 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/12/28 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #7672 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 70BG72086 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #7697 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 70YY27064 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/04/20 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #7514 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, 90BG08075 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2012/12/28 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE, DARK 	Drying time: 4 WEEKS, test #7671 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 19YR14629 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #8094 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 19YY51758 EARTH GLAZE 4 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, YELLOW 	Drying time: 4 WEEKS, test #8093 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 2070Y10R SUNBED 	ICI PAINTS (M) 	C BREWER & SONS (S) 	F 	2014/04/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, YELLOW 	Drying time: 4 WEEKS, test #8165 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 20YY23246 LABRADOR SANDS 1 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BROWN, LIGHT 	Drying time: 4 WEEKS, test #8049 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 20YY27225 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BEIGE 	Drying time: 4 WEEKS, test #8052 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 20YY34700 SUNDRENCHED SAFFRON 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, YELLOW 	Drying time: 4 WEEKS, test #8046 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 20YY54342 GOLDEN UMBER 3 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, YELLOW, LIGHT 	Drying time: 4 WEEKS, test #8103 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30BB08263 ATOMIC SURF 1 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8047 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30YR11393 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #8053 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30YR13471 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #8050 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 30YR14365 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, ORANGE 	Drying time: 4 WEEKS, test #8043 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 4040980Y 	ICI PAINTS (M) 	C BREWER & SONS (S) 	F 	2014/04/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #8170 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 43BB09340 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8044 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50BB08257 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8051 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50BB11216 MORNING JEWEL 1 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8045 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 50BB11321 SAPPHIRE SPRING 2 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8048 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70GY14187 TUSCAN GLADE 1 	ICI PAINTS (M) 	C BREWER & SONS (S) 	F 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #8090 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 70YY12167 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2013/11/14 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #8042 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 7500N 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/04/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #8166 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, 90GY16151 HIGHLAND FALLS 1 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREEN 	Drying time: 4 WEEKS, test #8091 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, S3060Y90R 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/04/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, RED 	Drying time: 4 WEEKS, test #8169 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 0500N JABOT 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/04/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, WHITE 	Drying time: 4 WEEKS, test #8167 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 10BG39244 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8100 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 10GG53030 HEBRIDEAN MISTS 4 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, LIGHT 	Drying time: 4 WEEKS, test #8099 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30BB45049 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY, LIGHT 	Drying time: 4 WEEKS, test #8098 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, LIGHT BASE, 30YY65171 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, CREAM 	Drying time: 4 WEEKS, test #8101 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 10BG22275 BLUE DIAMOND 3 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, TURQUOISE, DARK 	Drying time: 4 WEEKS, test #8107 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 16BG24357 BLUE DIAMOND 4 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, TURQUOISE 	Drying time: 4 WEEKS, test #8108 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 30BB31043 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, GREY 	Drying time: 4 WEEKS, test #8097 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 5020B309 TARN 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/04/04 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8168 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 50BG20230 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, BLUE 	Drying time: 4 WEEKS, test #8096 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 88GG32346 CRYSTAL SURPRISE 1 	ICI PAINTS (M) 	C BREWER & SONS (S) 	T 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, TURQUOISE 	Drying time: 4 WEEKS, test #8105 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, MEDIUM BASE, 90GG28133 SEA URCHIN 2 	ICI PAINTS (M) 	C BREWER & SONS (S) 	P 	2014/01/16 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, TURQUOISE 	Drying time: 4 WEEKS, test #8106 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, HOT PAPRIKA 1 R03 	ICI PAINTS (M) 	LEYLAND SDM (S) 	P 	2013/07/08 	BM 	Oddy Test 	VINYL EMULSION, RED, DARK 	Drying time: 5 WEEKS 4 DAYS, test #7898 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, HIMALAYAN MUSK 70RB11196 	ICI PAINTS (M) 	LEYLAND SDM (S) 	T 	2013/09/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, PURPLE, DARK 	Drying time: 4 WEEKS, test #7933 	COATING, PAINT 	none 	
DULUX TRADE VINYL MATT EMULSION, EXTRA DEEP BASE, VENETIAN CRYSTAL 10BB07150 	ICI PAINTS (M) 	LEYLAND SDM (S) 	T 	2013/09/10 	BM 	Oddy Test 	WATER BASED ACRYLIC COPOLYMER, TURQUOISE, DARK 	Drying time: 4 WEEKS, test #7934 	COATING, PAINT 	none 	
INTERCOAT PRIMER, 20846 	INTERCOAT (M) 	GOODFORD PTY LTD (S) 	P 	2013/12/30 	BM 	Oddy Test 	ACRYLIC EMULSION, WHITE 	Drying time: 4 WEEKS, test #8128 	COATING, PRIMER 	none 	
INTERCOAT SATIN ENAMEL, 12830 	INTERCOAT (M) 	GOODFORD PTY LTD (S) 	T 	2013/12/30 	BM 	Oddy Test 	ACRYLIC EMULSION, WHITE 	Drying time: 4 WEEKS, test #8127 	COATING, PAINT 	none 	
INTERCOAT SATIN ENAMEL, 12993 	INTERCOAT (M) 	GOODFORD PTY LTD (S) 	P 	2013/12/30 	BM 	Oddy Test 	ACRYLIC EMULSION, BLACK 	Drying time: 4 WEEKS, test #8129 	COATING, PAINT 	none 	
INTERNATIONAL 3 IN 1 PRIMER, SEALER, UNDERCOAT, 	INTERNATIONAL 	INTERNATIONAL 	F 	2009/06/29 	BM 	Oddy Test 	PETROLIUM BASED, WHITE 	Drying time: 4 WEEKS, test #6526 	COATING, PRIMER 	none 	
INTERNATIONAL EXTERIOR WOOD PRIMER, 	INTERNATIONAL 	INTERNATIONAL 	F 	2009/06/29 	BM 	Oddy Test 	PETROLIUM BASED, WHITE 	Drying time: 4 WEEKS, test #6527 	COATING, PRIMER 	none 	
INTERNATIONAL QUICK DRY FLOOR PAINT, PEBBLESTONE 	INTERNATIONAL 	INTERNATIONAL 	F 	2009/06/29 	BM 	Oddy Test 	PETROLIUM BASED, CREAM 	Drying time: 4 WEEKS, test #6536 	COATING, PAINT 	none 	
GARDEX PAINT, B LIGHT GREEN 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, GREEN, LIGHT 	Drying time: 4 WEEKS, test #7816 	COATING, PAINT 	none 	
GARDEX PAINT, BLACK 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, BLACK 	Drying time: 4 WEEKS, test #7817 	COATING, PAINT 	none 	
GARDEX PAINT, P298C DARK BEIGE 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, BEIGE 	Drying time: 4 WEEKS, test #7814 	COATING, PAINT 	none 	
GARDEX PAINT, P730C DARK BLUE 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, BLUE, DARK 	Drying time: 4 WEEKS, test #7813 	COATING, PAINT 	none 	
GARDEX PAINT, P7463C DARK GREEN 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, GREEN, DARK 	Drying time: 4 WEEKS, test #7812 	COATING, PAINT 	none 	
GARDEX PAINT, P7506C LIGHT BEIGE 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, BEIGE 	Drying time: 4 WEEKS, test #7811 	COATING, PAINT 	none 	
GARDEX PAINT, P7737C LIGHT BLUE 	JOTUN (M) 	UNKNOWN 	F 	2013/04/25 	BM 	Oddy Test 	SOLVENT BASED ALKYD ENAMEL + ACTIVE FUNGICIDE, BLUE, LIGHT 	Drying time: 4 WEEKS, test #7815 	COATING, PAINT 	none 	
COLOR XPRESS, ULTRA DEEP BASE, 10031 SPACE 	KALON DECORATIVE PRODUCTS (M) 	LEYLAND SDM (S) 	T 	2013/07/08 	BM 	Oddy Test 	VINYL EMULSION, BLUE, DARK 	Drying time: 5 WEEKS 4 DAYS, test #7899 	COATING, PAINT 	none 	
DULUX ENVIRO2 PROFESSIONAL INTERIOR LOW SHEEN , AUDD 1274 	KI PAINTS (M) 	DULUX AUSTRALIA (S) 	P 	2013/04/18 	BM 	Oddy Test 	ACRYLIC EMULSION, WHITE 	Drying time: 4 WEEKS, test #7766 	COATING, PAINT 	none 	
RUEGENER CHALK PAINT, 70514 20 	KREIDEWERK PUGER, PURE NATURE 	KREIDEWERK PUGER, PURE NATURE 	P 	2009/06/29 	BM 	Oddy Test 	CHALK, METHYLCELLULOSE, WHITE 	Drying time: 4 WEEKS, test #6518 	COATING, PAINT 	none 	
CASEIN MARBLE FLOUR PAINT, 70729 20 	KREIDEZEIT, PURE NATURE 	KREIDEZEIT, PURE NATURE 	P 	2009/06/29 	BM 	Oddy Test 	CASEIN, WHITE 	Drying time: 4 WEEKS, test #6528 	COATING, PAINT 	none 	
VEGA WALL PAINT, 70717 20 	KREIDEZEIT, PURE NATURE 	KREIDEZEIT, PURE NATURE 	P 	2009/06/29 	BM 	Oddy Test 	Marble flour, chalk, vegetable casein, kaoline, talcum, kieselguhr, lime hydrate, borax, soda, methyl cellulose, WHITE 	Drying time: 4 WEEKS, test #6519 	COATING, PAINT 	none 	
MS2A REDUCED KETONE RESIN, MS2A RESIN 	LINDEN CHEMICALS 	LINDEN CHEMICALS 	T 	2009/08/05 	BM 	Oddy Test 	Reduced Cyclic Ketone Polymer, CLEAR 	Drying time: 4 WEEKS, test #6589 	COATING, VARNISH 	none 	
MS2A REDUCED KETONE RESIN WITH TINUVIN 292 (LIGHT STABILIZER), MS2A RESIN + TINUVIN 292 	LINDEN CHEMICALS 	LINDEN CHEMICALS 	T 	2009/08/05 	BM 	Oddy Test 	Reduced Cyclic Ketone Polymer and light stablizer, CLEAR 	Drying time: 4 WEEKS, test #6590 	COATING, VARNISH 	none 	
LIQUITEX PROFESSIONAL, SERIES 1 244 IVORY BLACK 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLACK 	Drying time: 4 WEEKS, test #6393 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 1 432 TITANIUM WHITE 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, WHITE 	Drying time: 4 WEEKS, test #6395 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 1 530 BRONZE YELLOW 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW, DARK 	Drying time: 4 WEEKS, test #6394 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 1A 316 PHTHALOCYANINE BLUE 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLUE 	Drying time: 4 WEEKS, test #6385 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 1A 317 PHTHALOCYANINE GREEN 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, GREEN 	Drying time: 4 WEEKS, test #6386 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 1A 570 BRILLIANT BLUE 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, BLUE 	Drying time: 4 WEEKS, test #6387 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 1A 830 CADMIUM YELLOW MEDIUM 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, YELLOW 	Drying time: 4 WEEKS, test #6389 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 2 450 EMERALD GREEN 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, GREEN, DARK 	Drying time: 4 WEEKS, test #6391 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 2 510 CADMIUM RED LIGHT 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, RED 	Drying time: 4 WEEKS, test #6392 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES 3 114 QUINACRIDONE MAGENTA 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, PURPLE, DARK 	Drying time: 4 WEEKS, test #6390 	COATING, PAINT 	none 	
LIQUITEX PROFESSIONAL, SERIES1 186 DIOXAZINE PURPLE 	LIQUITEX 	LIQUITEX 	P 	2009/04/03 	BM 	Oddy Test 	ACRYLIC PAINT, PURPLE 	Drying time: 4 WEEKS, test #6388 	COATING, PAINT 	none 	
LITTLE GREENE ENGLISH HERITAGE ABSOLUTE EMULSION, BRONZE RED 15 	LITTLE GREENE 	LITTLE GREENE 	P 	2013/07/08 	BM 	Oddy Test 	VINYL EMULSION, RED 	Drying time: 5 WEEKS 4 DAYS, test #7900 	COATING, PAINT 	none 	
PYLOX SPRAY PAINT, 705 	NIPPON PAINT 	NIPPON PAINT 	F 	2013/04/25 	BM 	Oddy Test 	ACRYLIC MODIFIED ALKYD NITRO-CELLULOSE, GOLD 	Drying time: 4 WEEKS, test #7818 	COATING, PAINT 	none 	
SILICONE NOVABOND 2, S29306000 	NOVABOND 	NOVABOND 	F 	2009/01/20 	BM 	Oddy Test 	SILICONE, BLACK 	Drying time: 48 HOURS, test #6156 	SEALANT 	none 	
SUPER ECO EMUSLION, 1-11881 	NUTSHELL 	NUTSHELL 	F 	2009/06/29 	BM 	Oddy Test 	PAINT, WHITE 	Drying time: 4 WEEKS, test #6531 	COATING, PAINT 	none 	
POWDER COATING, RAL 7021, MATT 30% GLOSS 	OMNIKOTE 	OMNIKOTE 	P 	2013/10/30 	BM 	Oddy Test 	POLYESTER, GREY, DARK 	Drying time: BAKED, test #8037 	COATING, POWDER 	none 	
POWDER COATING, RAL 8500N, MATT 30% GLOSS 	OMNIKOTE 	OMNIKOTE 	P 	2013/10/30 	BM 	Oddy Test 	POLYESTER, BLACK 	Drying time: BAKED, test #8038 	COATING, POWDER 	none 	
POWDER COATING, RAL 9004 FINE TEXTURE 	OMNIKOTE 	OMNIKOTE 	P 	2013/10/30 	BM 	Oddy Test 	POLYESTER, BLACK 	Drying time: BAKED, test #8041 	COATING, POWDER 	none 	
POWDER COATING, RAL 9005, MATT 30% GLOSS 	OMNIKOTE 	OMNIKOTE 	P 	2013/10/30 	BM 	Oddy Test 	POLYESTER, BLACK 	Drying time: BAKED, test #8040 	COATING, POWDER 	none 	
POWDER COATING, RAL 9011, MATT 30% GLOSS 	OMNIKOTE 	OMNIKOTE 	P 	2013/10/30 	BM 	Oddy Test 	POLYESTER, BLACK 	Drying time: BAKED, test #8039 	COATING, POWDER 	none 	
PACTAN , 7042 1K 	PACTAN (M) 	UNKNOWN 	P 	2013/03/22 	BM 	Oddy Test 	SILICON, WHITE 	Drying time: 48 HOURS, test #7737 	SEALANT 	none 	
PACTAN , 8051 2K 	PACTAN (M) 	UNKNOWN 	P 	2013/03/22 	BM 	Oddy Test 	SILICON, WHITE 	Drying time: 48 HOURS, test #7736 	SEALANT 	none 	
JOHNSTONE'S TRADE COVAPLUS VINYL MATT EMULSION, 1710-1298BNTB27 	PPG INDUSTRIES (M) 	C BREWER AND SONS (S) 	P 	2013/01/19 	BM 	Oddy Test 	VINYL EMULSION, BLUE 	Drying time: 4 WEEKS, test #7685 	COATING, PAINT 	none 	
JOHNSTONE'S TRADE COVAPLUS VINYL MATT EMULSION, 3147-Y94R 	PPG INDUSTRIES (M) 	C BREWER AND SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	VINYL EMULSION, RED 	Drying time: 4 WEEKS, test #7700 	COATING, PAINT 	none 	
JOHNSTONE'S TRADE COVAPLUS VINYL MATT EMULSION, NEWTONS APPLE 	PPG INDUSTRIES (M) 	C BREWER AND SONS (S) 	P 	2013/02/11 	BM 	Oddy Test 	VINYL EMULSION, RED 	Drying time: 4 WEEKS, test #7701 	COATING, PAINT 	none 	
LEYLAND TRADE ACRYLIC EGGSHELL, PASTEL BASE, PASTEL BASE 	PPG INDUSTRIES (M) 	UNKNOWN 	P 	2009/02/12 	BM 	Oddy Test 	ACRYLIC, BEIGE 	Drying time: 4 WEEKS, test #6193 	COATING, PAINT 	none 	
LEYLAND TRADE VINYL MATT EMULSION, FIRE CRACKER 	PPG INDUSTRIES (M) 	UNKNOWN 	P 	2009/04/13 	BM 	Oddy Test 	ACRYLIC, RED 	Drying time: 4 WEEKS, test #6406 	COATING, PAINT 	none 	
LEYLAND TRADE VINYL MATT EMULSION, RAL 7043 	PPG INDUSTRIES (M) 	UNKNOWN 	P 	2009/02/13 	BM 	Oddy Test 	ACRYLIC, GREY, DARK 	Drying time: 4 WEEKS, test #6352 	COATING, PAINT 	none 	
GLUE BOUND WALL PAINT, 703301 20 	PURE NATURE 	PURE NATURE 	P 	2009/06/29 	BM 	Oddy Test 	CHALK, MAPLE POWDER , TALCUM, METHYLCELLULOSE CAOLINE, WHITE 	Drying time: 4 WEEKS, test #6529 	COATING, PAINT 	none 	
SANDERSON SPECTRUM PAINT, 42-27 T RIPE OLIVE TR 	SANDERSON (M) 	SIMPSONS PAINTS LONDON (S) 	P 	2011/03/22 	BM 	Oddy Test 	ACRYLIC EMULSION, GREEN 	Drying time: 4 WEEKS, test #7230 	COATING, PAINT 	none 	
SANDERSON SPECTRUM PAINT, 42-28 T, BARK MOSS TR 	SANDERSON (M) 	SIMPSONS PAINTS LONDON (S) 	P 	2011/03/22 	BM 	Oddy Test 	ACRYLIC EMULSION, GREEN 	Drying time: 4 WEEKS, test #7229 	COATING, PAINT 	none 	
Acoustical sealant 	Sheetrock 	Unknown 	Pass w/ reservations 	2000/03/21 	GCI 	Oddy 	sealant for walls 	apply as a paint 	sealant 	n/a 	
E27 100% ACRYLIC EMULSION, E27 	TECHNICAL PAINTS SERVICES 	TECHNICAL PAINTS SERVICES 	P 	2009/06/29 	BM 	Oddy Test 	ACRYLIC PAINT, WHITE 	Drying time: 4 WEEKS, test #6532 	COATING, PAINT 	none 	
MSP27 MULTISURFACE PRIMER, MSP27 	TECHNICAL PAINTS SERVICES 	TECHNICAL PAINTS SERVICES 	P 	2009/04/03 	BM 	Oddy Test 	PAINT, WHITE 	Drying time: 4 WEEKS, test #6359 	COATING, PRIMER 	none 	
MSP27 MULTISURFACE PRIMER, MSP27 	TECHNICAL PAINTS SERVICES 	TECHNICAL PAINTS SERVICES 	T 	2009/06/29 	BM 	Oddy Test 	, WHITE 	Drying time: 4 WEEKS, test #6525 	COATING, PRIMER 	none 	
RUST-OLEUM PAINTERS TOUCH, MATT SPRAY PAINT, AE0040028E8 	TOR COATINGS 	TOR COATINGS 	F 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, GREY, LIGHT 	Drying time: 4 WEEKS, test #6979 	COATING, PAINT 	none 	
RUST-OLEUM PAINTERS TOUCH, MATT SPRAY PAINT, AE0050005E8 	TOR COATINGS 	TOR COATINGS 	F 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, BLACK 	Drying time: 4 WEEKS, test #6980 	COATING, PAINT 	none 	
RUST-OLEUM PAINTERS TOUCH, MATT SPRAY PAINT, AE0050008E8 	TOR COATINGS 	TOR COATINGS 	F 	2010/09/16 	BM 	Oddy Test 	SOLVENT BASED AEROSOL, WHITE 	Drying time: 4 WEEKS, test #6981 	COATING, PAINT 	none 	
PolyWhey Furniture Clear Satin FNPTSG 	Vermont Natural Coatings 	Vermont Natural Coatings 	Fail 	2012/05/15 	CMA 	Oddy Test 	clear, satin/ whey based coating 	2 coats applied to Medex and allowed to dry 24 hours between coatings 	barrier, coating 	none 	
PolyWhey Furniture Gloss FNPTGL 	Vermont Natural Coatings 	Vermont Natural Coatings 	Fail 	2012/05/15 	CMA 	Oddy Test 	clear, glossy/ whey based coating 	2 coats applied to Medex and allowed to dry 24 hours between coatings 	barrier, coating 	none 	
WOOD VARNISH PRO AQUA, 70762 20 	VOLVOX 	VOLVOX 	P 	2009/06/29 	BM 	Oddy Test 	WATER BASED EMULSION, CLEAR 	Drying time: 4 WEEKS, test #6539 	COATING, VARNISH 	none 	
Uni-ball Signo DX 	- 	- 	PASS 	2017/08/16 	HCC 	Oddy Test 	BLACK 	Accessioning pen 	Gel Ink 	 	
Epocite 1004 T 	Polymer Technologies Pte. Ltd, Singapore 	- 	PASS 	2017/08/16 	HCC 	Oddy Test 	CLEAR 	Material gets yellow easily. For mounts with carbon fibre only. 	Epoxy 	 	
StoColor Sil In 	Sto SE & Co KGaA 	Sto SEA Pte. Ltd. Singapore 	PASS 	2018/08/23 	HCC 	Oddy Test 	Interior silicate paint used in public areas, colour white 	none 	Silicate Paint 	 	
StoPox BB T 200 	Sto SE & Co KGaA 	Sto SEA Pte. Ltd. Singapore 	PASS 	2018/08/23 	HCC 	Oddy Test 	Coating system for floors used in public areas, colour amber 	none 	Epoxy Terrazzo Coating System for Floors 	 	
Aqua Woodguard 	Nippon Paint 	--- 	PASS 	2019/02/14 	HCC 	Oddy Test 	Exterior wood varnish 	none 	--- 	100px 	
Agateen 	 	 	FAIL 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	CLEAR 	 	Cellulose Nitrate 	Link to Results PDF 	
Aura Paint, Cured 	Benjamin Moore 	 	PASS to Temporary 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Eggshell 	 	Polystyrene acrylate ester 	Link to Results PDF 	
Clean Seal Adhesive Teardrop Gasket 	 	 	PASS 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Black 	 	Polydimethylsiloxane 	Link to Results PDF 	
Fuhr Sealant 	 	 	PASS to Temporary 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Clear/White 	 	Polymer - sealant 	Link to Results PDF 	
RTV162 Silicone Caulk 	 	 	FAIL 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	White 	 	Polymer - Silicone Polydimethylsiloxane 	Link to Results PDF 	
Ultra Paint, Cured 	Benjamin Moore 	 	Temporary to FAIL 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Eggshell 	 	Elvace 1875 	Link to Results PDF 	
Window Gel 	 	 	FAIL 	2016/7 	IMA 	Oddy Test, Microchemical Tests, and EGA 	Orange 	 	Cellulose Propionate 	Link to Results PDF 	
==List of Manufacturers==
* Delta Design
* SheetRock
* Vermont Natural Coatings
==External Links==
* 'Sustainable Use of Coatings in Museums and Archives – Some Critical Observations' by Jean Tetreault 
Category:Exhibition
Category:Testing
Category:Choosing Materials